# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2014

#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_x

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Eu3 Na15 O36 Si12'
_chemical_formula_weight         1713.81

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Eu Eu -0.1578 3.6682 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   Pnnm

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'x+1/2, -y+1/2, -z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z'
'-x-1/2, y-1/2, z-1/2'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   10.7143(9)
_cell_length_b                   7.5271(7)
_cell_length_c                   10.4913(9)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_volume                     846.10(13)
_cell_formula_units_Z            1
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    4014
_cell_measurement_theta_min      5.48
_cell_measurement_theta_max      50.04

_exptl_crystal_description       sheet
_exptl_crystal_colour            corlourless
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.09
_exptl_crystal_size_min          0.05
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    3.363
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             810
_exptl_absorpt_coefficient_mu    6.244
_exptl_absorpt_correction_type   'Multi Scan'
_exptl_absorpt_correction_T_min  0.515
_exptl_absorpt_correction_T_max  0.732
_exptl_absorpt_process_details   ?

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  CCD
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            4014
_diffrn_reflns_av_R_equivalents  0.0192
_diffrn_reflns_av_sigmaI/netI    0.0138
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_theta_min         2.72
_diffrn_reflns_theta_max         25.02
_reflns_number_total             791
_reflns_number_gt                736
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    ?
_computing_publication_material  ?

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0850P)²+3.7000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   none
_refine_ls_hydrogen_treatment    none
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         791
_refine_ls_number_parameters     87
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0309
_refine_ls_R_factor_gt           0.0288
_refine_ls_wR_factor_ref         0.1094
_refine_ls_wR_factor_gt          0.1068
_refine_ls_goodness_of_fit_ref   1.004
_refine_ls_restrained_S_all      1.004
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Eu1 Eu 0.5000 1.0000 0.5000 0.0120(3) Uani 1 4 d S . .
Eu2 Eu 0.75180(17) 0.7657(2) 0.0000 0.0180(4) Uani 0.16 2 d SP . 1
Eu3 Eu 1.0000 1.0000 0.0000 0.0151(6) Uani 0.18 4 d SP . 1
Na2 Na 0.75180(17) 0.7657(2) 0.0000 0.0180(4) Uani 0.84 2 d SP . 2
Na3 Na 1.0000 1.0000 0.0000 0.0151(6) Uani 0.82 4 d SP . 2
Na1 Na 0.5000 1.0000 0.0000 0.051(2) Uani 1 4 d S . .
Na4 Na 0.7605(3) 0.5249(3) 0.2482(3) 0.0287(7) Uani 1 1 d . . .
Si1 Si 0.7871(2) 0.7600(2) 0.5000 0.0072(5) Uani 1 2 d S . .
Si2 Si 0.99109(12) 0.7870(2) 0.27635(17) 0.0078(4) Uani 1 1 d . . .
O1 O 0.7112(5) 0.9408(8) 0.5000 0.0272(14) Uani 1 2 d S . .
O2 O 0.7084(5) 0.5816(7) 0.5000 0.0229(13) Uani 1 2 d S . .
O3 O 0.8790(5) 0.7503(7) 0.3791(5) 0.0432(15) Uani 1 1 d . . .
O4 O 0.9405(4) 0.7150(5) 0.1428(4) 0.0247(10) Uani 1 1 d . . .
O5 O 1.0000 1.0000 0.2600(8) 0.057(3) Uani 1 2 d S . .
O6 O 1.1172(4) 0.7089(7) 0.3258(4) 0.0354(12) Uani 1 1 d . . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Eu1 O4 2.295(4) 3_465 ?
Eu1 O4 2.295(4) 7_766 ?
Eu1 O4 2.295(4) 8_576 ?
Eu1 O4 2.295(4) 4_655 ?
Eu1 O1 2.307(5) . ?
Eu1 O1 2.307(5) 5_676 ?
Eu1 Eu2 3.3272(16) 3_465 ?
Eu1 Na2 3.3272(16) 3_465 ?
Eu1 Na2 3.3272(16) 7_766 ?
Eu1 Eu2 3.3272(16) 7_766 ?
Eu1 Si1 3.567(2) . ?
Eu1 Si1 3.567(2) 5_676 ?
Eu2 O6 2.336(4) 8_575 ?
Eu2 O6 2.336(4) 3_465 ?
Eu2 O2 2.416(6) 7_765 ?
Eu2 O1 2.477(6) 7_755 ?
Eu2 O4 2.545(4) . ?
Eu2 O4 2.545(4) 6 ?
Eu2 Na4 3.173(3) 6 ?
Eu2 Na4 3.173(3) . ?
Eu2 Eu3 3.1910(18) . ?
Eu2 Na1 3.2233(17) . ?
Eu2 Na4 3.287(3) 4_655 ?
Eu2 Na4 3.287(3) 7_765 ?
Eu3 O2 2.316(5) 3_565 ?
Eu3 O2 2.316(5) 7_765 ?
Eu3 O4 2.693(4) 6 ?
Eu3 O4 2.693(4) 2_775 ?
Eu3 O4 2.693(4) . ?
Eu3 O4 2.693(4) 5_775 ?
Eu3 O5 2.727(9) 5_775 ?
Eu3 O5 2.727(9) . ?
Eu3 Eu2 3.1910(18) 5_775 ?
Eu3 Si2 3.3144(18) 6 ?
Eu3 Si2 3.3144(18) 2_775 ?
Na1 O3 2.615(6) 8_575 ?
Na1 O3 2.615(6) 4_655 ?
Na1 O3 2.615(6) 3_465 ?
Na1 O3 2.615(6) 7_765 ?
Na1 O6 2.719(6) 8_575 ?
Na1 O6 2.719(6) 3_465 ?
Na1 O6 2.719(6) 4_655 ?
Na1 O6 2.719(6) 7_765 ?
Na1 Si1 3.005(2) 3_465 ?
Na1 Si1 3.005(2) 7_765 ?
Na1 Si2 3.1909(18) 8_575 ?
Na1 Si2 3.1909(18) 4_655 ?
Na4 O6 2.341(5) 2_765 ?
Na4 O3 2.525(5) . ?
Na4 O6 2.641(6) 3_465 ?
Na4 O4 2.643(5) . ?
Na4 O1 2.696(3) 7_755 ?
Na4 O2 2.734(3) . ?
Na4 O5 2.799(3) 3_465 ?
Na4 O3 2.880(6) 4_645 ?
Na4 Si2 3.175(3) . ?
Na4 Si1 3.192(3) . ?
Si1 O1 1.585(6) . ?
Si1 O2 1.586(5) . ?
Si1 O3 1.608(4) 6_556 ?
Si1 O3 1.608(4) . ?
Si1 Na1 3.005(2) 3_565 ?
Si1 Na4 3.192(3) 6_556 ?
Si1 Na4 3.319(3) 7_766 ?
Si1 Na4 3.319(3) 4_655 ?
Si1 Eu3 3.646(2) 3_465 ?
Si2 O6 1.562(4) . ?
Si2 O4 1.597(4) . ?
Si2 O5 1.615(2) . ?
Si2 O3 1.637(4) . ?
Si2 Na1 3.1909(18) 3_565 ?
Si2 Na4 3.226(3) 3_565 ?
Si2 Na4 3.247(3) 4_655 ?
Si2 Eu1 3.6169(18) 3_565 ?
Si2 Eu2 3.670(2) 3_565 ?
O1 Na2 2.477(6) 7_766 ?
O1 Eu2 2.477(6) 7_766 ?
O1 Na4 2.696(3) 7_766 ?
O1 Na4 2.696(3) 4_655 ?
O2 Na3 2.316(5) 3_465 ?
O2 Eu3 2.316(5) 3_465 ?
O2 Na2 2.416(6) 7_756 ?
O2 Eu2 2.416(6) 7_756 ?
O2 Na4 2.734(3) 6_556 ?
O3 Na1 2.615(6) 3_565 ?
O3 Na4 2.880(6) 4_655 ?
O4 Eu1 2.295(4) 3_565 ?
O5 Si2 1.615(2) 2_775 ?
O5 Na4 2.799(3) 4_655 ?
O5 Na4 2.799(3) 3_565 ?
O6 Na2 2.336(4) 3_565 ?
O6 Eu2 2.336(4) 3_565 ?
O6 Na4 2.341(5) 2_765 ?
O6 Na4 2.641(6) 3_565 ?
O6 Na1 2.719(6) 3_565 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O4 Eu1 O4 180.000(1) 3_465 7_766 ?
O4 Eu1 O4 81.5(2) 3_465 8_576 ?
O4 Eu1 O4 98.5(2) 7_766 8_576 ?
O4 Eu1 O4 98.5(2) 3_465 4_655 ?
O4 Eu1 O4 81.5(2) 7_766 4_655 ?
O4 Eu1 O4 180.00(14) 8_576 4_655 ?
O4 Eu1 O1 97.83(15) 3_465 . ?
O4 Eu1 O1 82.17(16) 7_766 . ?
O4 Eu1 O1 97.83(15) 8_576 . ?
O4 Eu1 O1 82.17(16) 4_655 . ?
O4 Eu1 O1 82.17(16) 3_465 5_676 ?
O4 Eu1 O1 97.83(15) 7_766 5_676 ?
O4 Eu1 O1 82.17(16) 8_576 5_676 ?
O4 Eu1 O1 97.83(15) 4_655 5_676 ?
O1 Eu1 O1 180.000(1) . 5_676 ?
O4 Eu1 Eu2 49.80(10) 3_465 3_465 ?
O4 Eu1 Eu2 130.20(10) 7_766 3_465 ?
O4 Eu1 Eu2 49.80(10) 8_576 3_465 ?
O4 Eu1 Eu2 130.20(10) 4_655 3_465 ?
O1 Eu1 Eu2 131.92(15) . 3_465 ?
O1 Eu1 Eu2 48.08(15) 5_676 3_465 ?
O4 Eu1 Na2 49.80(10) 3_465 3_465 ?
O4 Eu1 Na2 130.20(10) 7_766 3_465 ?
O4 Eu1 Na2 49.80(10) 8_576 3_465 ?
O4 Eu1 Na2 130.20(10) 4_655 3_465 ?
O1 Eu1 Na2 131.92(15) . 3_465 ?
O1 Eu1 Na2 48.08(15) 5_676 3_465 ?
Eu2 Eu1 Na2 0.00(4) 3_465 3_465 ?
O4 Eu1 Na2 130.20(10) 3_465 7_766 ?
O4 Eu1 Na2 49.80(10) 7_766 7_766 ?
O4 Eu1 Na2 130.20(10) 8_576 7_766 ?
O4 Eu1 Na2 49.80(10) 4_655 7_766 ?
O1 Eu1 Na2 48.08(15) . 7_766 ?
O1 Eu1 Na2 131.92(15) 5_676 7_766 ?
Eu2 Eu1 Na2 180.0 3_465 7_766 ?
Na2 Eu1 Na2 180.0 3_465 7_766 ?
O4 Eu1 Eu2 130.20(10) 3_465 7_766 ?
O4 Eu1 Eu2 49.80(10) 7_766 7_766 ?
O4 Eu1 Eu2 130.20(10) 8_576 7_766 ?
O4 Eu1 Eu2 49.80(10) 4_655 7_766 ?
O1 Eu1 Eu2 48.08(15) . 7_766 ?
O1 Eu1 Eu2 131.92(15) 5_676 7_766 ?
Eu2 Eu1 Eu2 180.0 3_465 7_766 ?
Na2 Eu1 Eu2 180.0 3_465 7_766 ?
Na2 Eu1 Eu2 0.00(4) 7_766 7_766 ?
O4 Eu1 Si1 83.24(11) 3_465 . ?
O4 Eu1 Si1 96.76(11) 7_766 . ?
O4 Eu1 Si1 83.24(11) 8_576 . ?
O4 Eu1 Si1 96.76(11) 4_655 . ?
O1 Eu1 Si1 19.29(15) . . ?
O1 Eu1 Si1 160.71(15) 5_676 . ?
Eu2 Eu1 Si1 112.63(4) 3_465 . ?
Na2 Eu1 Si1 112.63(4) 3_465 . ?
Na2 Eu1 Si1 67.37(4) 7_766 . ?
Eu2 Eu1 Si1 67.37(4) 7_766 . ?
O4 Eu1 Si1 96.76(11) 3_465 5_676 ?
O4 Eu1 Si1 83.24(11) 7_766 5_676 ?
O4 Eu1 Si1 96.76(11) 8_576 5_676 ?
O4 Eu1 Si1 83.24(11) 4_655 5_676 ?
O1 Eu1 Si1 160.71(15) . 5_676 ?
O1 Eu1 Si1 19.29(15) 5_676 5_676 ?
Eu2 Eu1 Si1 67.37(4) 3_465 5_676 ?
Na2 Eu1 Si1 67.37(4) 3_465 5_676 ?
Na2 Eu1 Si1 112.63(4) 7_766 5_676 ?
Eu2 Eu1 Si1 112.63(4) 7_766 5_676 ?
Si1 Eu1 Si1 180.0 . 5_676 ?
O6 Eu2 O6 103.0(3) 8_575 3_465 ?
O6 Eu2 O2 91.63(14) 8_575 7_765 ?
O6 Eu2 O2 91.63(14) 3_465 7_765 ?
O6 Eu2 O1 100.34(16) 8_575 7_755 ?
O6 Eu2 O1 100.34(16) 3_465 7_755 ?
O2 Eu2 O1 160.6(2) 7_765 7_755 ?
O6 Eu2 O4 164.42(17) 8_575 . ?
O6 Eu2 O4 92.42(16) 3_465 . ?
O2 Eu2 O4 90.42(15) 7_765 . ?
O1 Eu2 O4 74.04(14) 7_755 . ?
O6 Eu2 O4 92.42(16) 8_575 6 ?
O6 Eu2 O4 164.42(17) 3_465 6 ?
O2 Eu2 O4 90.42(15) 7_765 6 ?
O1 Eu2 O4 74.04(14) 7_755 6 ?
O4 Eu2 O4 72.11(19) . 6 ?
O6 Eu2 Na4 54.76(15) 8_575 6 ?
O6 Eu2 Na4 134.98(13) 3_465 6 ?
O2 Eu2 Na4 123.83(5) 7_765 6 ?
O1 Eu2 Na4 55.36(5) 7_755 6 ?
O4 Eu2 Na4 111.95(11) . 6 ?
O4 Eu2 Na4 53.71(11) 6 6 ?
O6 Eu2 Na4 134.98(13) 8_575 . ?
O6 Eu2 Na4 54.76(15) 3_465 . ?
O2 Eu2 Na4 123.83(5) 7_765 . ?
O1 Eu2 Na4 55.36(5) 7_755 . ?
O4 Eu2 Na4 53.71(11) . . ?
O4 Eu2 Na4 111.95(11) 6 . ?
Na4 Eu2 Na4 110.26(9) 6 . ?
O6 Eu2 Eu3 117.99(11) 8_575 . ?
O6 Eu2 Eu3 117.99(11) 3_465 . ?
O2 Eu2 Eu3 46.28(13) 7_765 . ?
O1 Eu2 Eu3 114.36(14) 7_755 . ?
O4 Eu2 Eu3 54.61(10) . . ?
O4 Eu2 Eu3 54.61(10) 6 . ?
Na4 Eu2 Eu3 106.92(6) 6 . ?
Na4 Eu2 Eu3 106.92(6) . . ?
O6 Eu2 Na1 55.84(14) 8_575 . ?
O6 Eu2 Na1 55.84(14) 3_465 . ?
O2 Eu2 Na1 66.99(13) 7_765 . ?
O1 Eu2 Na1 132.37(14) 7_755 . ?
O4 Eu2 Na1 138.33(9) . . ?
O4 Eu2 Na1 138.33(9) 6 . ?
Na4 Eu2 Na1 109.70(6) 6 . ?
Na4 Eu2 Na1 109.70(6) . . ?
Eu3 Eu2 Na1 113.27(4) . . ?
O6 Eu2 Na4 123.74(16) 8_575 4_655 ?
O6 Eu2 Na4 45.40(11) 3_465 4_655 ?
O2 Eu2 Na4 54.74(5) 7_765 4_655 ?
O1 Eu2 Na4 126.33(5) 7_755 4_655 ?
O4 Eu2 Na4 69.39(10) . 4_655 ?
O4 Eu2 Na4 126.44(13) 6 4_655 ?
Na4 Eu2 Na4 178.27(9) 6 4_655 ?
Na4 Eu2 Na4 71.384(8) . 4_655 ?
Eu3 Eu2 Na4 72.87(5) . 4_655 ?
Na1 Eu2 Na4 68.99(5) . 4_655 ?
O6 Eu2 Na4 45.40(11) 8_575 7_765 ?
O6 Eu2 Na4 123.74(16) 3_465 7_765 ?
O2 Eu2 Na4 54.74(5) 7_765 7_765 ?
O1 Eu2 Na4 126.33(5) 7_755 7_765 ?
O4 Eu2 Na4 126.44(13) . 7_765 ?
O4 Eu2 Na4 69.39(10) 6 7_765 ?
Na4 Eu2 Na4 71.384(9) 6 7_765 ?
Na4 Eu2 Na4 178.27(9) . 7_765 ?
Eu3 Eu2 Na4 72.87(5) . 7_765 ?
Na1 Eu2 Na4 68.99(5) . 7_765 ?
Na4 Eu2 Na4 106.97(9) 4_655 7_765 ?
O2 Eu3 O2 180.0 3_565 7_765 ?
O2 Eu3 O4 90.97(15) 3_565 6 ?
O2 Eu3 O4 89.03(15) 7_765 6 ?
O2 Eu3 O4 89.03(15) 3_565 2_775 ?
O2 Eu3 O4 90.97(15) 7_765 2_775 ?
O4 Eu3 O4 180.00(13) 6 2_775 ?
O2 Eu3 O4 90.97(15) 3_565 . ?
O2 Eu3 O4 89.03(15) 7_765 . ?
O4 Eu3 O4 67.60(15) 6 . ?
O4 Eu3 O4 112.40(15) 2_775 . ?
O2 Eu3 O4 89.03(15) 3_565 5_775 ?
O2 Eu3 O4 90.97(15) 7_765 5_775 ?
O4 Eu3 O4 112.40(15) 6 5_775 ?
O4 Eu3 O4 67.60(15) 2_775 5_775 ?
O4 Eu3 O4 180.00(10) . 5_775 ?
O2 Eu3 O5 90.000(1) 3_565 5_775 ?
O2 Eu3 O5 90.000(1) 7_765 5_775 ?
O4 Eu3 O5 56.20(8) 6 5_775 ?
O4 Eu3 O5 123.80(8) 2_775 5_775 ?
O4 Eu3 O5 123.80(8) . 5_775 ?
O4 Eu3 O5 56.20(8) 5_775 5_775 ?
O2 Eu3 O5 90.0 3_565 . ?
O2 Eu3 O5 90.0 7_765 . ?
O4 Eu3 O5 123.80(8) 6 . ?
O4 Eu3 O5 56.20(8) 2_775 . ?
O4 Eu3 O5 56.20(8) . . ?
O4 Eu3 O5 123.80(8) 5_775 . ?
O5 Eu3 O5 180.000(1) 5_775 . ?
O2 Eu3 Eu2 131.07(14) 3_565 . ?
O2 Eu3 Eu2 48.93(14) 7_765 . ?
O4 Eu3 Eu2 50.40(9) 6 . ?
O4 Eu3 Eu2 129.60(9) 2_775 . ?
O4 Eu3 Eu2 50.40(9) . . ?
O4 Eu3 Eu2 129.60(9) 5_775 . ?
O5 Eu3 Eu2 90.0 5_775 . ?
O5 Eu3 Eu2 90.0 . . ?
O2 Eu3 Eu2 48.93(14) 3_565 5_775 ?
O2 Eu3 Eu2 131.07(14) 7_765 5_775 ?
O4 Eu3 Eu2 129.60(9) 6 5_775 ?
O4 Eu3 Eu2 50.40(9) 2_775 5_775 ?
O4 Eu3 Eu2 129.60(9) . 5_775 ?
O4 Eu3 Eu2 50.40(9) 5_775 5_775 ?
O5 Eu3 Eu2 90.0 5_775 5_775 ?
O5 Eu3 Eu2 90.0 . 5_775 ?
Eu2 Eu3 Eu2 180.0 . 5_775 ?
O2 Eu3 Si2 84.23(7) 3_565 6 ?
O2 Eu3 Si2 95.77(7) 7_765 6 ?
O4 Eu3 Si2 28.51(8) 6 6 ?
O4 Eu3 Si2 151.49(8) 2_775 6 ?
O4 Eu3 Si2 95.42(8) . 6 ?
O4 Eu3 Si2 84.58(8) 5_775 6 ?
O5 Eu3 Si2 28.98(3) 5_775 6 ?
O5 Eu3 Si2 151.02(3) . 6 ?
Eu2 Eu3 Si2 73.06(3) . 6 ?
Eu2 Eu3 Si2 106.94(3) 5_775 6 ?
O2 Eu3 Si2 95.77(7) 3_565 2_775 ?
O2 Eu3 Si2 84.23(7) 7_765 2_775 ?
O4 Eu3 Si2 151.49(8) 6 2_775 ?
O4 Eu3 Si2 28.51(8) 2_775 2_775 ?
O4 Eu3 Si2 84.58(8) . 2_775 ?
O4 Eu3 Si2 95.42(8) 5_775 2_775 ?
O5 Eu3 Si2 151.02(3) 5_775 2_775 ?
O5 Eu3 Si2 28.98(3) . 2_775 ?
Eu2 Eu3 Si2 106.94(3) . 2_775 ?
Eu2 Eu3 Si2 73.06(3) 5_775 2_775 ?
Si2 Eu3 Si2 180.00(6) 6 2_775 ?
O3 Na1 O3 180.00(18) 8_575 4_655 ?
O3 Na1 O3 58.04(19) 8_575 3_465 ?
O3 Na1 O3 121.96(19) 4_655 3_465 ?
O3 Na1 O3 121.96(19) 8_575 7_765 ?
O3 Na1 O3 58.04(19) 4_655 7_765 ?
O3 Na1 O3 180.0 3_465 7_765 ?
O3 Na1 O6 59.07(14) 8_575 8_575 ?
O3 Na1 O6 120.93(14) 4_655 8_575 ?
O3 Na1 O6 97.95(13) 3_465 8_575 ?
O3 Na1 O6 82.05(13) 7_765 8_575 ?
O3 Na1 O6 97.95(13) 8_575 3_465 ?
O3 Na1 O6 82.05(13) 4_655 3_465 ?
O3 Na1 O6 59.07(14) 3_465 3_465 ?
O3 Na1 O6 120.93(14) 7_765 3_465 ?
O6 Na1 O6 84.49(18) 8_575 3_465 ?
O3 Na1 O6 120.93(14) 8_575 4_655 ?
O3 Na1 O6 59.07(14) 4_655 4_655 ?
O3 Na1 O6 82.05(13) 3_465 4_655 ?
O3 Na1 O6 97.95(13) 7_765 4_655 ?
O6 Na1 O6 180.0 8_575 4_655 ?
O6 Na1 O6 95.51(18) 3_465 4_655 ?
O3 Na1 O6 82.05(13) 8_575 7_765 ?
O3 Na1 O6 97.95(13) 4_655 7_765 ?
O3 Na1 O6 120.93(14) 3_465 7_765 ?
O3 Na1 O6 59.07(14) 7_765 7_765 ?
O6 Na1 O6 95.51(18) 8_575 7_765 ?
O6 Na1 O6 180.0 3_465 7_765 ?
O6 Na1 O6 84.49(18) 4_655 7_765 ?
O3 Na1 Si1 32.30(9) 8_575 3_465 ?
O3 Na1 Si1 147.70(9) 4_655 3_465 ?
O3 Na1 Si1 32.30(9) 3_465 3_465 ?
O3 Na1 Si1 147.70(9) 7_765 3_465 ?
O6 Na1 Si1 88.50(9) 8_575 3_465 ?
O6 Na1 Si1 88.50(9) 3_465 3_465 ?
O6 Na1 Si1 91.50(9) 4_655 3_465 ?
O6 Na1 Si1 91.50(9) 7_765 3_465 ?
O3 Na1 Si1 147.70(9) 8_575 7_765 ?
O3 Na1 Si1 32.30(9) 4_655 7_765 ?
O3 Na1 Si1 147.70(9) 3_465 7_765 ?
O3 Na1 Si1 32.30(9) 7_765 7_765 ?
O6 Na1 Si1 91.50(9) 8_575 7_765 ?
O6 Na1 Si1 91.50(9) 3_465 7_765 ?
O6 Na1 Si1 88.50(9) 4_655 7_765 ?
O6 Na1 Si1 88.50(9) 7_765 7_765 ?
Si1 Na1 Si1 180.0 3_465 7_765 ?
O3 Na1 Si2 30.76(10) 8_575 8_575 ?
O3 Na1 Si2 149.24(10) 4_655 8_575 ?
O3 Na1 Si2 81.61(10) 3_465 8_575 ?
O3 Na1 Si2 98.39(10) 7_765 8_575 ?
O6 Na1 Si2 29.28(9) 8_575 8_575 ?
O6 Na1 Si2 96.69(10) 3_465 8_575 ?
O6 Na1 Si2 150.72(9) 4_655 8_575 ?
O6 Na1 Si2 83.31(10) 7_765 8_575 ?
Si1 Na1 Si2 62.38(4) 3_465 8_575 ?
Si1 Na1 Si2 117.62(4) 7_765 8_575 ?
O3 Na1 Si2 149.24(10) 8_575 4_655 ?
O3 Na1 Si2 30.76(10) 4_655 4_655 ?
O3 Na1 Si2 98.39(10) 3_465 4_655 ?
O3 Na1 Si2 81.61(10) 7_765 4_655 ?
O6 Na1 Si2 150.72(9) 8_575 4_655 ?
O6 Na1 Si2 83.31(10) 3_465 4_655 ?
O6 Na1 Si2 29.28(9) 4_655 4_655 ?
O6 Na1 Si2 96.69(10) 7_765 4_655 ?
Si1 Na1 Si2 117.62(4) 3_465 4_655 ?
Si1 Na1 Si2 62.38(4) 7_765 4_655 ?
Si2 Na1 Si2 180.00(4) 8_575 4_655 ?
O6 Na4 O3 92.0(2) 2_765 . ?
O6 Na4 O6 176.63(13) 2_765 3_465 ?
O3 Na4 O6 86.72(18) . 3_465 ?
O6 Na4 O4 98.29(17) 2_765 . ?
O3 Na4 O4 59.81(14) . . ?
O6 Na4 O4 83.74(15) 3_465 . ?
O6 Na4 O1 95.54(19) 2_765 7_755 ?
O3 Na4 O1 128.80(19) . 7_755 ?
O6 Na4 O1 87.68(18) 3_465 7_755 ?
O4 Na4 O1 69.00(16) . 7_755 ?
O6 Na4 O2 83.99(18) 2_765 . ?
O3 Na4 O2 58.15(16) . . ?
O6 Na4 O2 92.69(17) 3_465 . ?
O4 Na4 O2 117.96(16) . . ?
O1 Na4 O2 173.04(19) 7_755 . ?
O6 Na4 O5 121.21(18) 2_765 3_465 ?
O3 Na4 O5 124.27(19) . 3_465 ?
O6 Na4 O5 57.44(12) 3_465 3_465 ?
O4 Na4 O5 138.69(19) . 3_465 ?
O1 Na4 O5 93.8(2) 7_755 3_465 ?
O2 Na4 O5 80.6(2) . 3_465 ?
O6 Na4 O3 84.95(18) 2_765 4_645 ?
O3 Na4 O3 174.60(16) . 4_645 ?
O6 Na4 O3 96.10(16) 3_465 4_645 ?
O4 Na4 O3 125.00(15) . 4_645 ?
O1 Na4 O3 56.08(15) 7_755 4_645 ?
O2 Na4 O3 116.99(17) . 4_645 ?
O5 Na4 O3 54.53(15) 3_465 4_645 ?
O6 Na4 Eu2 137.01(15) 2_765 . ?
O3 Na4 Eu2 94.45(14) . . ?
O6 Na4 Eu2 46.26(11) 3_465 . ?
O4 Na4 Eu2 50.91(10) . . ?
O1 Na4 Eu2 49.10(13) 7_755 . ?
O2 Na4 Eu2 134.25(14) . . ?
O5 Na4 Eu2 89.08(17) 3_465 . ?
O3 Na4 Eu2 90.82(11) 4_645 . ?
O6 Na4 Si2 89.97(16) 2_765 . ?
O3 Na4 Si2 30.77(10) . . ?
O6 Na4 Si2 90.49(11) 3_465 . ?
O4 Na4 Si2 30.13(9) . . ?
O1 Na4 Si2 98.55(15) 7_755 . ?
O2 Na4 Si2 88.40(13) . . ?
O5 Na4 Si2 145.13(9) 3_465 . ?
O3 Na4 Si2 153.29(14) 4_645 . ?
Eu2 Na4 Si2 75.20(8) . . ?
O6 Na4 Si1 94.53(16) 2_765 . ?
O3 Na4 Si1 29.86(11) . . ?
O6 Na4 Si1 82.80(12) 3_465 . ?
O4 Na4 Si1 88.92(11) . . ?
O1 Na4 Si1 156.82(16) 7_755 . ?
O2 Na4 Si1 29.77(11) . . ?
O5 Na4 Si1 98.70(18) 3_465 . ?
O3 Na4 Si1 145.87(13) 4_645 . ?
Eu2 Na4 Si1 111.42(8) . . ?
Si2 Na4 Si1 60.61(6) . . ?
O1 Si1 O2 117.0(3) . . ?
O1 Si1 O3 110.7(2) . 6_556 ?
O2 Si1 O3 106.7(2) . 6_556 ?
O1 Si1 O3 110.7(2) . . ?
O2 Si1 O3 106.7(2) . . ?
O3 Si1 O3 104.2(4) 6_556 . ?
O1 Si1 Na1 161.5(2) . 3_565 ?
O2 Si1 Na1 81.5(2) . 3_565 ?
O3 Si1 Na1 60.4(2) 6_556 3_565 ?
O3 Si1 Na1 60.4(2) . 3_565 ?
O1 Si1 Na4 115.47(11) . . ?
O2 Si1 Na4 58.89(8) . . ?
O3 Si1 Na4 133.0(2) 6_556 . ?
O3 Si1 Na4 51.42(18) . . ?
Na1 Si1 Na4 72.95(6) 3_565 . ?
O1 Si1 Na4 115.47(11) . 6_556 ?
O2 Si1 Na4 58.89(8) . 6_556 ?
O3 Si1 Na4 51.42(18) 6_556 6_556 ?
O3 Si1 Na4 133.0(2) . 6_556 ?
Na1 Si1 Na4 72.95(6) 3_565 6_556 ?
Na4 Si1 Na4 111.71(11) . 6_556 ?
O1 Si1 Na4 53.50(7) . 7_766 ?
O2 Si1 Na4 115.28(12) . 7_766 ?
O3 Si1 Na4 60.2(2) 6_556 7_766 ?
O3 Si1 Na4 137.8(2) . 7_766 ?
Na1 Si1 Na4 120.53(7) 3_565 7_766 ?
Na4 Si1 Na4 165.57(8) . 7_766 ?
Na4 Si1 Na4 70.737(11) 6_556 7_766 ?
O1 Si1 Na4 53.50(7) . 4_655 ?
O2 Si1 Na4 115.28(12) . 4_655 ?
O3 Si1 Na4 137.8(2) 6_556 4_655 ?
O3 Si1 Na4 60.2(2) . 4_655 ?
Na1 Si1 Na4 120.53(7) 3_565 4_655 ?
Na4 Si1 Na4 70.737(11) . 4_655 ?
Na4 Si1 Na4 165.57(8) 6_556 4_655 ?
Na4 Si1 Na4 103.33(11) 7_766 4_655 ?
O1 Si1 Eu1 28.7(2) . . ?
O2 Si1 Eu1 88.3(2) . . ?
O3 Si1 Eu1 123.5(2) 6_556 . ?
O3 Si1 Eu1 123.5(2) . . ?
Na1 Si1 Eu1 169.80(7) 3_565 . ?
Na4 Si1 Eu1 101.76(6) . . ?
Na4 Si1 Eu1 101.76(6) 6_556 . ?
Na4 Si1 Eu1 64.09(6) 7_766 . ?
Na4 Si1 Eu1 64.09(6) 4_655 . ?
O1 Si1 Eu3 91.6(2) . 3_465 ?
O2 Si1 Eu3 25.4(2) . 3_465 ?
O3 Si1 Eu3 119.51(18) 6_556 3_465 ?
O3 Si1 Eu3 119.51(18) . 3_465 ?
Na1 Si1 Eu3 106.91(5) 3_565 3_465 ?
Na4 Si1 Eu3 68.12(6) . 3_465 ?
Na4 Si1 Eu3 68.12(6) 6_556 3_465 ?
Na4 Si1 Eu3 101.11(6) 7_766 3_465 ?
Na4 Si1 Eu3 101.11(6) 4_655 3_465 ?
Eu1 Si1 Eu3 62.89(4) . 3_465 ?
O6 Si2 O4 117.2(2) . . ?
O6 Si2 O5 111.0(2) . . ?
O4 Si2 O5 105.3(3) . . ?
O6 Si2 O3 110.6(3) . . ?
O4 Si2 O3 105.8(3) . . ?
O5 Si2 O3 106.3(3) . . ?
O6 Si2 Na4 118.0(2) . . ?
O4 Si2 Na4 56.18(17) . . ?
O5 Si2 Na4 130.75(11) . . ?
O3 Si2 Na4 52.10(18) . . ?
O6 Si2 Na1 58.3(2) . 3_565 ?
O4 Si2 Na1 115.18(17) . 3_565 ?
O5 Si2 Na1 138.5(3) . 3_565 ?
O3 Si2 Na1 54.8(2) . 3_565 ?
Na4 Si2 Na1 70.80(6) . 3_565 ?
O6 Si2 Na4 54.4(2) . 3_565 ?
O4 Si2 Na4 112.49(18) . 3_565 ?
O5 Si2 Na4 60.20(7) . 3_565 ?
O3 Si2 Na4 141.5(2) . 3_565 ?
Na4 Si2 Na4 164.06(8) . 3_565 ?
Na1 Si2 Na4 109.20(7) 3_565 3_565 ?
O6 Si2 Na4 162.18(18) . 4_655 ?
O4 Si2 Na4 80.57(17) . 4_655 ?
O5 Si2 Na4 59.55(6) . 4_655 ?
O3 Si2 Na4 62.4(2) . 4_655 ?
Na4 Si2 Na4 71.90(3) . 4_655 ?
Na1 Si2 Na4 117.16(7) 3_565 4_655 ?
Na4 Si2 Na4 119.66(8) 3_565 4_655 ?
O6 Si2 Eu3 116.6(2) . . ?
O4 Si2 Eu3 53.60(16) . . ?
O5 Si2 Eu3 54.9(3) . . ?
O3 Si2 Eu3 132.7(2) . . ?
Na4 Si2 Eu3 103.97(7) . . ?
Na1 Si2 Eu3 165.90(6) 3_565 . ?
Na4 Si2 Eu3 72.08(6) 3_565 . ?
Na4 Si2 Eu3 71.81(6) 4_655 . ?
O6 Si2 Eu1 91.07(17) . 3_565 ?
O4 Si2 Eu1 26.22(15) . 3_565 ?
O5 Si2 Eu1 120.4(3) . 3_565 ?
O3 Si2 Eu1 116.50(18) . 3_565 ?
Na4 Si2 Eu1 64.83(6) . 3_565 ?
Na1 Si2 Eu1 100.62(5) 3_565 3_565 ?
Na4 Si2 Eu1 100.05(6) 3_565 3_565 ?
Na4 Si2 Eu1 106.73(6) 4_655 3_565 ?
Eu3 Si2 Eu1 65.60(3) . 3_565 ?
O6 Si2 Eu2 24.29(16) . 3_565 ?
O4 Si2 Eu2 141.49(17) . 3_565 ?
O5 Si2 Eu2 97.5(2) . 3_565 ?
O3 Si2 Eu2 96.8(2) . 3_565 ?
Na4 Si2 Eu2 125.78(7) . 3_565 ?
Na1 Si2 Eu2 55.52(3) 3_565 3_565 ?
Na4 Si2 Eu2 54.34(6) 3_565 3_565 ?
Na4 Si2 Eu2 137.93(7) 4_655 3_565 ?
Eu3 Si2 Eu2 126.13(4) . 3_565 ?
Eu1 Si2 Eu2 115.34(5) 3_565 3_565 ?
Si1 O1 Eu1 132.0(3) . . ?
Si1 O1 Na2 140.0(3) . 7_766 ?
Eu1 O1 Na2 88.06(19) . 7_766 ?
Si1 O1 Eu2 140.0(3) . 7_766 ?
Eu1 O1 Eu2 88.06(19) . 7_766 ?
Na2 O1 Eu2 0.000(11) 7_766 7_766 ?
Si1 O1 Na4 98.29(14) . 7_766 ?
Eu1 O1 Na4 93.70(14) . 7_766 ?
Na2 O1 Na4 75.54(13) 7_766 7_766 ?
Eu2 O1 Na4 75.54(13) 7_766 7_766 ?
Si1 O1 Na4 98.29(14) . 4_655 ?
Eu1 O1 Na4 93.70(14) . 4_655 ?
Na2 O1 Na4 75.54(13) 7_766 4_655 ?
Eu2 O1 Na4 75.54(13) 7_766 4_655 ?
Na4 O1 Na4 149.8(3) 7_766 4_655 ?
Si1 O2 Na3 137.5(3) . 3_465 ?
Si1 O2 Eu3 137.5(3) . 3_465 ?
Na3 O2 Eu3 0.0 3_465 3_465 ?
Si1 O2 Na2 137.7(3) . 7_756 ?
Na3 O2 Na2 84.79(18) 3_465 7_756 ?
Eu3 O2 Na2 84.79(18) 3_465 7_756 ?
Si1 O2 Eu2 137.7(3) . 7_756 ?
Na3 O2 Eu2 84.79(18) 3_465 7_756 ?
Eu3 O2 Eu2 84.79(18) 3_465 7_756 ?
Na2 O2 Eu2 0.000(12) 7_756 7_756 ?
Si1 O2 Na4 91.34(13) . 6_556 ?
Na3 O2 Na4 98.96(13) 3_465 6_556 ?
Eu3 O2 Na4 98.96(13) 3_465 6_556 ?
Na2 O2 Na4 79.08(13) 7_756 6_556 ?
Eu2 O2 Na4 79.08(13) 7_756 6_556 ?
Si1 O2 Na4 91.34(13) . . ?
Na3 O2 Na4 98.96(13) 3_465 . ?
Eu3 O2 Na4 98.96(13) 3_465 . ?
Na2 O2 Na4 79.08(13) 7_756 . ?
Eu2 O2 Na4 79.08(13) 7_756 . ?
Na4 O2 Na4 150.2(3) 6_556 . ?
Si1 O3 Si2 164.0(3) . . ?
Si1 O3 Na4 98.7(2) . . ?
Si2 O3 Na4 97.1(2) . . ?
Si1 O3 Na1 87.3(2) . 3_565 ?
Si2 O3 Na1 94.5(2) . 3_565 ?
Na4 O3 Na1 91.67(17) . 3_565 ?
Si1 O3 Na4 90.9(2) . 4_655 ?
Si2 O3 Na4 87.4(2) . 4_655 ?
Na4 O3 Na4 88.22(17) . 4_655 ?
Na1 O3 Na4 178.16(19) 3_565 4_655 ?
Si2 O4 Eu1 135.9(2) . 3_565 ?
Si2 O4 Eu2 137.3(2) . . ?
Eu1 O4 Eu2 86.67(12) 3_565 . ?
Si2 O4 Na4 93.7(2) . . ?
Eu1 O4 Na4 95.39(15) 3_565 . ?
Eu2 O4 Na4 75.38(14) . . ?
Si2 O4 Eu3 97.90(19) . . ?
Eu1 O4 Eu3 97.63(14) 3_565 . ?
Eu2 O4 Eu3 75.00(11) . . ?
Na4 O4 Eu3 146.75(18) . . ?
Si2 O5 Si2 167.8(6) . 2_775 ?
Si2 O5 Eu3 96.1(3) . . ?
Si2 O5 Eu3 96.1(3) 2_775 . ?
Si2 O5 Na4 90.62(7) . 4_655 ?
Si2 O5 Na4 89.75(7) 2_775 4_655 ?
Eu3 O5 Na4 88.3(2) . 4_655 ?
Si2 O5 Na4 89.75(7) . 3_565 ?
Si2 O5 Na4 90.62(7) 2_775 3_565 ?
Eu3 O5 Na4 88.3(2) . 3_565 ?
Na4 O5 Na4 176.5(4) 4_655 3_565 ?
Si2 O6 Na2 139.7(3) . 3_565 ?
Si2 O6 Eu2 139.7(3) . 3_565 ?
Na2 O6 Eu2 0.0 3_565 3_565 ?
Si2 O6 Na4 130.7(3) . 2_765 ?
Na2 O6 Na4 89.33(16) 3_565 2_765 ?
Eu2 O6 Na4 89.33(16) 3_565 2_765 ?
Si2 O6 Na4 96.9(2) . 3_565 ?
Na2 O6 Na4 78.97(16) 3_565 3_565 ?
Eu2 O6 Na4 78.97(16) 3_565 3_565 ?
Na4 O6 Na4 98.21(17) 2_765 3_565 ?
Si2 O6 Na1 92.4(2) . 3_565 ?
Na2 O6 Na1 78.84(15) 3_565 3_565 ?
Eu2 O6 Na1 78.84(15) 3_565 3_565 ?
Na4 O6 Na1 93.28(18) 2_765 3_565 ?
Na4 O6 Na1 154.83(19) 3_565 3_565 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O6 Eu2 Eu3 O2 -117.62(16) 8_575 . . 3_565 ?
O6 Eu2 Eu3 O2 117.62(16) 3_465 . . 3_565 ?
O2 Eu2 Eu3 O2 180.0 7_765 . . 3_565 ?
O1 Eu2 Eu3 O2 0.0 7_755 . . 3_565 ?
O4 Eu2 Eu3 O2 46.22(11) . . . 3_565 ?
O4 Eu2 Eu3 O2 -46.22(11) 6 . . 3_565 ?
Na4 Eu2 Eu3 O2 -59.04(5) 6 . . 3_565 ?
Na4 Eu2 Eu3 O2 59.04(5) . . . 3_565 ?
Na1 Eu2 Eu3 O2 180.0 . . . 3_565 ?
Na4 Eu2 Eu3 O2 122.75(5) 4_655 . . 3_565 ?
Na4 Eu2 Eu3 O2 -122.75(5) 7_765 . . 3_565 ?
O6 Eu2 Eu3 O2 62.38(16) 8_575 . . 7_765 ?
O6 Eu2 Eu3 O2 -62.38(16) 3_465 . . 7_765 ?
O1 Eu2 Eu3 O2 180.0 7_755 . . 7_765 ?
O4 Eu2 Eu3 O2 -133.78(11) . . . 7_765 ?
O4 Eu2 Eu3 O2 133.78(11) 6 . . 7_765 ?
Na4 Eu2 Eu3 O2 120.96(5) 6 . . 7_765 ?
Na4 Eu2 Eu3 O2 -120.96(5) . . . 7_765 ?
Na1 Eu2 Eu3 O2 0.0 . . . 7_765 ?
Na4 Eu2 Eu3 O2 -57.25(5) 4_655 . . 7_765 ?
Na4 Eu2 Eu3 O2 57.25(5) 7_765 . . 7_765 ?
O6 Eu2 Eu3 O4 -71.40(19) 8_575 . . 6 ?
O6 Eu2 Eu3 O4 163.8(2) 3_465 . . 6 ?
O2 Eu2 Eu3 O4 -133.78(11) 7_765 . . 6 ?
O1 Eu2 Eu3 O4 46.22(11) 7_755 . . 6 ?
O4 Eu2 Eu3 O4 92.4(2) . . . 6 ?
Na4 Eu2 Eu3 O4 -12.82(11) 6 . . 6 ?
Na4 Eu2 Eu3 O4 105.26(12) . . . 6 ?
Na1 Eu2 Eu3 O4 -133.78(11) . . . 6 ?
Na4 Eu2 Eu3 O4 168.97(12) 4_655 . . 6 ?
Na4 Eu2 Eu3 O4 -76.53(11) 7_765 . . 6 ?
O6 Eu2 Eu3 O4 108.60(19) 8_575 . . 2_775 ?
O6 Eu2 Eu3 O4 -16.2(2) 3_465 . . 2_775 ?
O2 Eu2 Eu3 O4 46.22(11) 7_765 . . 2_775 ?
O1 Eu2 Eu3 O4 -133.78(11) 7_755 . . 2_775 ?
O4 Eu2 Eu3 O4 -87.6(2) . . . 2_775 ?
O4 Eu2 Eu3 O4 180.0 6 . . 2_775 ?
Na4 Eu2 Eu3 O4 167.18(11) 6 . . 2_775 ?
Na4 Eu2 Eu3 O4 -74.74(12) . . . 2_775 ?
Na1 Eu2 Eu3 O4 46.22(11) . . . 2_775 ?
Na4 Eu2 Eu3 O4 -11.03(12) 4_655 . . 2_775 ?
Na4 Eu2 Eu3 O4 103.47(11) 7_765 . . 2_775 ?
O6 Eu2 Eu3 O4 -163.8(2) 8_575 . . . ?
O6 Eu2 Eu3 O4 71.40(19) 3_465 . . . ?
O2 Eu2 Eu3 O4 133.78(11) 7_765 . . . ?
O1 Eu2 Eu3 O4 -46.22(11) 7_755 . . . ?
O4 Eu2 Eu3 O4 -92.4(2) 6 . . . ?
Na4 Eu2 Eu3 O4 -105.26(12) 6 . . . ?
Na4 Eu2 Eu3 O4 12.82(11) . . . . ?
Na1 Eu2 Eu3 O4 133.78(11) . . . . ?
Na4 Eu2 Eu3 O4 76.53(11) 4_655 . . . ?
Na4 Eu2 Eu3 O4 -168.97(12) 7_765 . . . ?
O6 Eu2 Eu3 O4 16.2(2) 8_575 . . 5_775 ?
O6 Eu2 Eu3 O4 -108.60(19) 3_465 . . 5_775 ?
O2 Eu2 Eu3 O4 -46.22(11) 7_765 . . 5_775 ?
O1 Eu2 Eu3 O4 133.78(11) 7_755 . . 5_775 ?
O4 Eu2 Eu3 O4 180.0 . . . 5_775 ?
O4 Eu2 Eu3 O4 87.6(2) 6 . . 5_775 ?
Na4 Eu2 Eu3 O4 74.74(12) 6 . . 5_775 ?
Na4 Eu2 Eu3 O4 -167.18(11) . . . 5_775 ?
Na1 Eu2 Eu3 O4 -46.22(11) . . . 5_775 ?
Na4 Eu2 Eu3 O4 -103.47(11) 4_655 . . 5_775 ?
Na4 Eu2 Eu3 O4 11.03(12) 7_765 . . 5_775 ?
O6 Eu2 Eu3 O5 -27.62(16) 8_575 . . 5_775 ?
O6 Eu2 Eu3 O5 -152.38(16) 3_465 . . 5_775 ?
O2 Eu2 Eu3 O5 -90.0 7_765 . . 5_775 ?
O1 Eu2 Eu3 O5 90.0 7_755 . . 5_775 ?
O4 Eu2 Eu3 O5 136.22(11) . . . 5_775 ?
O4 Eu2 Eu3 O5 43.78(11) 6 . . 5_775 ?
Na4 Eu2 Eu3 O5 30.96(5) 6 . . 5_775 ?
Na4 Eu2 Eu3 O5 149.04(5) . . . 5_775 ?
Na1 Eu2 Eu3 O5 -90.0 . . . 5_775 ?
Na4 Eu2 Eu3 O5 -147.25(5) 4_655 . . 5_775 ?
Na4 Eu2 Eu3 O5 -32.75(5) 7_765 . . 5_775 ?
O6 Eu2 Eu3 O5 152.38(16) 8_575 . . . ?
O6 Eu2 Eu3 O5 27.62(16) 3_465 . . . ?
O2 Eu2 Eu3 O5 90.0 7_765 . . . ?
O1 Eu2 Eu3 O5 -90.0 7_755 . . . ?
O4 Eu2 Eu3 O5 -43.78(11) . . . . ?
O4 Eu2 Eu3 O5 -136.22(11) 6 . . . ?
Na4 Eu2 Eu3 O5 -149.04(5) 6 . . . ?
Na4 Eu2 Eu3 O5 -30.96(5) . . . . ?
Na1 Eu2 Eu3 O5 90.0 . . . . ?
Na4 Eu2 Eu3 O5 32.75(5) 4_655 . . . ?
Na4 Eu2 Eu3 O5 147.25(5) 7_765 . . . ?
O6 Eu2 Eu3 Eu2 62.38(16) 8_575 . . 5_775 ?
O6 Eu2 Eu3 Eu2 -62.38(16) 3_465 . . 5_775 ?
O2 Eu2 Eu3 Eu2 0.0 7_765 . . 5_775 ?
O1 Eu2 Eu3 Eu2 180.0 7_755 . . 5_775 ?
O4 Eu2 Eu3 Eu2 -133.78(11) . . . 5_775 ?
O4 Eu2 Eu3 Eu2 133.78(11) 6 . . 5_775 ?
Na4 Eu2 Eu3 Eu2 120.96(5) 6 . . 5_775 ?
Na4 Eu2 Eu3 Eu2 -120.96(5) . . . 5_775 ?
Na1 Eu2 Eu3 Eu2 0.0 . . . 5_775 ?
Na4 Eu2 Eu3 Eu2 -57.25(5) 4_655 . . 5_775 ?
Na4 Eu2 Eu3 Eu2 57.25(5) 7_765 . . 5_775 ?
O6 Eu2 Eu3 Si2 -51.50(17) 8_575 . . 6 ?
O6 Eu2 Eu3 Si2 -176.25(17) 3_465 . . 6 ?
O2 Eu2 Eu3 Si2 -113.87(3) 7_765 . . 6 ?
O1 Eu2 Eu3 Si2 66.13(3) 7_755 . . 6 ?
O4 Eu2 Eu3 Si2 112.35(11) . . . 6 ?
O4 Eu2 Eu3 Si2 19.90(11) 6 . . 6 ?
Na4 Eu2 Eu3 Si2 7.08(5) 6 . . 6 ?
Na4 Eu2 Eu3 Si2 125.17(7) . . . 6 ?
Na1 Eu2 Eu3 Si2 -113.87(3) . . . 6 ?
Na4 Eu2 Eu3 Si2 -171.12(7) 4_655 . . 6 ?
Na4 Eu2 Eu3 Si2 -56.63(5) 7_765 . . 6 ?
O6 Eu2 Eu3 Si2 128.50(17) 8_575 . . 2_775 ?
O6 Eu2 Eu3 Si2 3.75(17) 3_465 . . 2_775 ?
O2 Eu2 Eu3 Si2 66.13(3) 7_765 . . 2_775 ?
O1 Eu2 Eu3 Si2 -113.87(3) 7_755 . . 2_775 ?
O4 Eu2 Eu3 Si2 -67.65(11) . . . 2_775 ?
O4 Eu2 Eu3 Si2 -160.10(11) 6 . . 2_775 ?
Na4 Eu2 Eu3 Si2 -172.92(5) 6 . . 2_775 ?
Na4 Eu2 Eu3 Si2 -54.83(7) . . . 2_775 ?
Na1 Eu2 Eu3 Si2 66.13(3) . . . 2_775 ?
Na4 Eu2 Eu3 Si2 8.88(7) 4_655 . . 2_775 ?
Na4 Eu2 Eu3 Si2 123.37(5) 7_765 . . 2_775 ?
O6 Eu2 Na4 O6 109.7(4) 8_575 . . 2_765 ?
O6 Eu2 Na4 O6 -178.9(3) 3_465 . . 2_765 ?
O2 Eu2 Na4 O6 -114.4(3) 7_765 . . 2_765 ?
O1 Eu2 Na4 O6 42.1(3) 7_755 . . 2_765 ?
O4 Eu2 Na4 O6 -53.2(3) . . . 2_765 ?
O4 Eu2 Na4 O6 -8.2(3) 6 . . 2_765 ?
Na4 Eu2 Na4 O6 49.7(3) 6 . . 2_765 ?
Eu3 Eu2 Na4 O6 -66.2(3) . . . 2_765 ?
Na1 Eu2 Na4 O6 170.6(2) . . . 2_765 ?
Na4 Eu2 Na4 O6 -130.9(3) 4_655 . . 2_765 ?
Na4 Eu2 Na4 O6 -149(2) 7_765 . . 2_765 ?
O6 Eu2 Na4 O3 -152.6(2) 8_575 . . . ?
O6 Eu2 Na4 O3 -81.15(19) 3_465 . . . ?
O2 Eu2 Na4 O3 -16.7(2) 7_765 . . . ?
O1 Eu2 Na4 O3 139.8(2) 7_755 . . . ?
O4 Eu2 Na4 O3 44.51(16) . . . . ?
O4 Eu2 Na4 O3 89.53(17) 6 . . . ?
Na4 Eu2 Na4 O3 147.42(13) 6 . . . ?
Eu3 Eu2 Na4 O3 31.54(14) . . . . ?
Na1 Eu2 Na4 O3 -91.65(14) . . . . ?
Na4 Eu2 Na4 O3 -33.16(12) 4_655 . . . ?
Na4 Eu2 Na4 O3 -51(2) 7_765 . . . ?
O6 Eu2 Na4 O6 -71.5(3) 8_575 . . 3_465 ?
O2 Eu2 Na4 O6 64.4(2) 7_765 . . 3_465 ?
O1 Eu2 Na4 O6 -139.0(2) 7_755 . . 3_465 ?
O4 Eu2 Na4 O6 125.66(18) . . . 3_465 ?
O4 Eu2 Na4 O6 170.68(18) 6 . . 3_465 ?
Na4 Eu2 Na4 O6 -131.43(15) 6 . . 3_465 ?
Eu3 Eu2 Na4 O6 112.69(13) . . . 3_465 ?
Na1 Eu2 Na4 O6 -10.51(13) . . . 3_465 ?
Na4 Eu2 Na4 O6 47.99(13) 4_655 . . 3_465 ?
Na4 Eu2 Na4 O6 30(2) 7_765 . . 3_465 ?
O6 Eu2 Na4 O4 162.9(2) 8_575 . . . ?
O6 Eu2 Na4 O4 -125.66(18) 3_465 . . . ?
O2 Eu2 Na4 O4 -61.2(2) 7_765 . . . ?
O1 Eu2 Na4 O4 95.32(19) 7_755 . . . ?
O4 Eu2 Na4 O4 45.02(15) 6 . . . ?
Na4 Eu2 Na4 O4 102.91(14) 6 . . . ?
Eu3 Eu2 Na4 O4 -12.97(11) . . . . ?
Na1 Eu2 Na4 O4 -136.17(12) . . . . ?
Na4 Eu2 Na4 O4 -77.67(13) 4_655 . . . ?
Na4 Eu2 Na4 O4 -96(2) 7_765 . . . ?
O6 Eu2 Na4 O1 67.5(3) 8_575 . . 7_755 ?
O6 Eu2 Na4 O1 139.0(2) 3_465 . . 7_755 ?
O2 Eu2 Na4 O1 -156.5(2) 7_765 . . 7_755 ?
O4 Eu2 Na4 O1 -95.32(19) . . . 7_755 ?
O4 Eu2 Na4 O1 -50.3(2) 6 . . 7_755 ?
Na4 Eu2 Na4 O1 7.59(19) 6 . . 7_755 ?
Eu3 Eu2 Na4 O1 -108.29(16) . . . 7_755 ?
Na1 Eu2 Na4 O1 128.51(17) . . . 7_755 ?
Na4 Eu2 Na4 O1 -172.99(19) 4_655 . . 7_755 ?
Na4 Eu2 Na4 O1 169(2) 7_765 . . 7_755 ?
O6 Eu2 Na4 O2 -104.2(3) 8_575 . . . ?
O6 Eu2 Na4 O2 -32.7(2) 3_465 . . . ?
O2 Eu2 Na4 O2 31.7(4) 7_765 . . . ?
O1 Eu2 Na4 O2 -171.7(3) 7_755 . . . ?
O4 Eu2 Na4 O2 93.0(2) . . . . ?
O4 Eu2 Na4 O2 138.0(2) 6 . . . ?
Na4 Eu2 Na4 O2 -164.12(17) 6 . . . ?
Eu3 Eu2 Na4 O2 80.0(2) . . . . ?
Na1 Eu2 Na4 O2 -43.2(2) . . . . ?
Na4 Eu2 Na4 O2 15.31(17) 4_655 . . . ?
Na4 Eu2 Na4 O2 -3(2) 7_765 . . . ?
O6 Eu2 Na4 O5 -28.3(2) 8_575 . . 3_465 ?
O6 Eu2 Na4 O5 43.16(17) 3_465 . . 3_465 ?
O2 Eu2 Na4 O5 107.6(2) 7_765 . . 3_465 ?
O1 Eu2 Na4 O5 -95.9(2) 7_755 . . 3_465 ?
O4 Eu2 Na4 O5 168.82(17) . . . 3_465 ?
O4 Eu2 Na4 O5 -146.17(16) 6 . . 3_465 ?
Na4 Eu2 Na4 O5 -88.27(15) 6 . . 3_465 ?
Eu3 Eu2 Na4 O5 155.85(12) . . . 3_465 ?
Na1 Eu2 Na4 O5 32.65(13) . . . 3_465 ?
Na4 Eu2 Na4 O5 91.15(14) 4_655 . . 3_465 ?
Na4 Eu2 Na4 O5 73(2) 7_765 . . 3_465 ?
O6 Eu2 Na4 O3 26.2(2) 8_575 . . 4_645 ?
O6 Eu2 Na4 O3 97.67(18) 3_465 . . 4_645 ?
O2 Eu2 Na4 O3 162.10(19) 7_765 . . 4_645 ?
O1 Eu2 Na4 O3 -41.35(18) 7_755 . . 4_645 ?
O4 Eu2 Na4 O3 -136.67(16) . . . 4_645 ?
O4 Eu2 Na4 O3 -91.66(16) 6 . . 4_645 ?
Na4 Eu2 Na4 O3 -33.77(15) 6 . . 4_645 ?
Eu3 Eu2 Na4 O3 -149.64(11) . . . 4_645 ?
Na1 Eu2 Na4 O3 87.16(11) . . . 4_645 ?
Na4 Eu2 Na4 O3 145.66(15) 4_655 . . 4_645 ?
Na4 Eu2 Na4 O3 128(2) 7_765 . . 4_645 ?
O6 Eu2 Na4 Si2 -176.8(2) 8_575 . . . ?
O6 Eu2 Na4 Si2 -105.37(14) 3_465 . . . ?
O2 Eu2 Na4 Si2 -40.94(18) 7_765 . . . ?
O1 Eu2 Na4 Si2 115.61(17) 7_755 . . . ?
O4 Eu2 Na4 Si2 20.29(11) . . . . ?
O4 Eu2 Na4 Si2 65.30(12) 6 . . . ?
Na4 Eu2 Na4 Si2 123.20(8) 6 . . . ?
Eu3 Eu2 Na4 Si2 7.32(6) . . . . ?
Na1 Eu2 Na4 Si2 -115.88(6) . . . . ?
Na4 Eu2 Na4 Si2 -57.38(6) 4_655 . . . ?
Na4 Eu2 Na4 Si2 -75(2) 7_765 . . . ?
O6 Eu2 Na4 Si1 -127.3(2) 8_575 . . . ?
O6 Eu2 Na4 Si1 -55.83(15) 3_465 . . . ?
O2 Eu2 Na4 Si1 8.6(2) 7_765 . . . ?
O1 Eu2 Na4 Si1 165.15(19) 7_755 . . . ?
O4 Eu2 Na4 Si1 69.83(13) . . . . ?
O4 Eu2 Na4 Si1 114.85(13) 6 . . . ?
Na4 Eu2 Na4 Si1 172.74(5) 6 . . . ?
Eu3 Eu2 Na4 Si1 56.86(9) . . . . ?
Na1 Eu2 Na4 Si1 -66.33(10) . . . . ?
Na4 Eu2 Na4 Si1 -7.84(6) 4_655 . . . ?
Na4 Eu2 Na4 Si1 -26(2) 7_765 . . . ?
O6 Na4 Si1 O1 -177.0(3) 2_765 . . . ?
O3 Na4 Si1 O1 96.9(4) . . . . ?
O6 Na4 Si1 O1 0.9(2) 3_465 . . . ?
O4 Na4 Si1 O1 84.8(2) . . . . ?
O1 Na4 Si1 O1 67.4(6) 7_755 . . . ?
O2 Na4 Si1 O1 -107.5(4) . . . . ?
O5 Na4 Si1 O1 -54.5(3) 3_465 . . . ?
O3 Na4 Si1 O1 -89.3(3) 4_645 . . . ?
Eu2 Na4 Si1 O1 38.0(2) . . . . ?
Si2 Na4 Si1 O1 95.6(2) . . . . ?
O6 Na4 Si1 O2 -69.5(3) 2_765 . . . ?
O3 Na4 Si1 O2 -155.6(4) . . . . ?
O6 Na4 Si1 O2 108.4(3) 3_465 . . . ?
O4 Na4 Si1 O2 -167.8(3) . . . . ?
O1 Na4 Si1 O2 174.9(4) 7_755 . . . ?
O5 Na4 Si1 O2 53.0(3) 3_465 . . . ?
O3 Na4 Si1 O2 18.2(3) 4_645 . . . ?
Eu2 Na4 Si1 O2 145.5(3) . . . . ?
Si2 Na4 Si1 O2 -156.9(3) . . . . ?
O6 Na4 Si1 O3 14.5(3) 2_765 . . 6_556 ?
O3 Na4 Si1 O3 -71.6(4) . . . 6_556 ?
O6 Na4 Si1 O3 -167.6(3) 3_465 . . 6_556 ?
O4 Na4 Si1 O3 -83.7(3) . . . 6_556 ?
O1 Na4 Si1 O3 -101.1(5) 7_755 . . 6_556 ?
O2 Na4 Si1 O3 84.0(4) . . . 6_556 ?
O5 Na4 Si1 O3 137.0(3) 3_465 . . 6_556 ?
O3 Na4 Si1 O3 102.2(4) 4_645 . . 6_556 ?
Eu2 Na4 Si1 O3 -130.5(3) . . . 6_556 ?
Si2 Na4 Si1 O3 -72.9(3) . . . 6_556 ?
O6 Na4 Si1 O3 86.1(3) 2_765 . . . ?
O6 Na4 Si1 O3 -96.0(3) 3_465 . . . ?
O4 Na4 Si1 O3 -12.1(3) . . . . ?
O1 Na4 Si1 O3 -29.5(5) 7_755 . . . ?
O2 Na4 Si1 O3 155.6(4) . . . . ?
O5 Na4 Si1 O3 -151.4(3) 3_465 . . . ?
O3 Na4 Si1 O3 173.8(3) 4_645 . . . ?
Eu2 Na4 Si1 O3 -58.9(3) . . . . ?
Si2 Na4 Si1 O3 -1.3(3) . . . . ?
O6 Na4 Si1 Na1 20.74(13) 2_765 . . 3_565 ?
O3 Na4 Si1 Na1 -65.4(3) . . . 3_565 ?
O6 Na4 Si1 Na1 -161.33(12) 3_465 . . 3_565 ?
O4 Na4 Si1 Na1 -77.50(11) . . . 3_565 ?
O1 Na4 Si1 Na1 -94.8(4) 7_755 . . 3_565 ?
O2 Na4 Si1 Na1 90.3(2) . . . 3_565 ?
O5 Na4 Si1 Na1 143.28(14) 3_465 . . 3_565 ?
O3 Na4 Si1 Na1 108.4(2) 4_645 . . 3_565 ?
Eu2 Na4 Si1 Na1 -124.28(9) . . . 3_565 ?
Si2 Na4 Si1 Na1 -66.68(6) . . . 3_565 ?
O6 Na4 Si1 Na4 -42.38(19) 2_765 . . 6_556 ?
O3 Na4 Si1 Na4 -128.5(3) . . . 6_556 ?
O6 Na4 Si1 Na4 135.55(12) 3_465 . . 6_556 ?
O4 Na4 Si1 Na4 -140.62(11) . . . 6_556 ?
O1 Na4 Si1 Na4 -157.9(4) 7_755 . . 6_556 ?
O2 Na4 Si1 Na4 27.1(3) . . . 6_556 ?
O5 Na4 Si1 Na4 80.17(15) 3_465 . . 6_556 ?
O3 Na4 Si1 Na4 45.3(3) 4_645 . . 6_556 ?
Eu2 Na4 Si1 Na4 172.60(5) . . . 6_556 ?
Si2 Na4 Si1 Na4 -129.79(10) . . . 6_556 ?
O6 Na4 Si1 Na4 -139.4(4) 2_765 . . 7_766 ?
O3 Na4 Si1 Na4 134.5(5) . . . 7_766 ?
O6 Na4 Si1 Na4 38.5(4) 3_465 . . 7_766 ?
O4 Na4 Si1 Na4 122.3(4) . . . 7_766 ?
O1 Na4 Si1 Na4 105.0(5) 7_755 . . 7_766 ?
O2 Na4 Si1 Na4 -69.9(5) . . . 7_766 ?
O5 Na4 Si1 Na4 -16.9(5) 3_465 . . 7_766 ?
O3 Na4 Si1 Na4 -51.7(6) 4_645 . . 7_766 ?
Eu2 Na4 Si1 Na4 75.6(4) . . . 7_766 ?
Si2 Na4 Si1 Na4 133.2(4) . . . 7_766 ?
O6 Na4 Si1 Na4 152.80(18) 2_765 . . 4_655 ?
O3 Na4 Si1 Na4 66.7(3) . . . 4_655 ?
O6 Na4 Si1 Na4 -29.26(10) 3_465 . . 4_655 ?
O4 Na4 Si1 Na4 54.57(11) . . . 4_655 ?
O1 Na4 Si1 Na4 37.3(4) 7_755 . . 4_655 ?
O2 Na4 Si1 Na4 -137.7(3) . . . 4_655 ?
O5 Na4 Si1 Na4 -84.65(14) 3_465 . . 4_655 ?
O3 Na4 Si1 Na4 -119.5(3) 4_645 . . 4_655 ?
Eu2 Na4 Si1 Na4 7.79(5) . . . 4_655 ?
Si2 Na4 Si1 Na4 65.39(8) . . . 4_655 ?
O6 Na4 Si1 Eu1 -150.26(14) 2_765 . . . ?
O3 Na4 Si1 Eu1 123.7(3) . . . . ?
O6 Na4 Si1 Eu1 27.68(11) 3_465 . . . ?
O4 Na4 Si1 Eu1 111.51(11) . . . . ?
O1 Na4 Si1 Eu1 94.2(4) 7_755 . . . ?
O2 Na4 Si1 Eu1 -80.7(2) . . . . ?
O5 Na4 Si1 Eu1 -27.71(13) 3_465 . . . ?
O3 Na4 Si1 Eu1 -62.6(2) 4_645 . . . ?
Eu2 Na4 Si1 Eu1 64.73(9) . . . . ?
Si2 Na4 Si1 Eu1 122.33(6) . . . . ?
O6 Na4 Si1 Eu3 -96.07(14) 2_765 . . 3_465 ?
O3 Na4 Si1 Eu3 177.8(3) . . . 3_465 ?
O6 Na4 Si1 Eu3 81.86(11) 3_465 . . 3_465 ?
O4 Na4 Si1 Eu3 165.69(12) . . . 3_465 ?
O1 Na4 Si1 Eu3 148.4(4) 7_755 . . 3_465 ?
O2 Na4 Si1 Eu3 -26.6(2) . . . 3_465 ?
O5 Na4 Si1 Eu3 26.47(12) 3_465 . . 3_465 ?
O3 Na4 Si1 Eu3 -8.4(2) 4_645 . . 3_465 ?
Eu2 Na4 Si1 Eu3 118.91(9) . . . 3_465 ?
Si2 Na4 Si1 Eu3 176.51(7) . . . 3_465 ?
O4 Eu1 Si1 O1 138.91(10) 3_465 . . . ?
O4 Eu1 Si1 O1 -41.09(10) 7_766 . . . ?
O4 Eu1 Si1 O1 -138.91(10) 8_576 . . . ?
O4 Eu1 Si1 O1 41.09(10) 4_655 . . . ?
O1 Eu1 Si1 O1 180.0 5_676 . . . ?
Eu2 Eu1 Si1 O1 180.0 3_465 . . . ?
Na2 Eu1 Si1 O1 180.0 3_465 . . . ?
Na2 Eu1 Si1 O1 0.0 7_766 . . . ?
Eu2 Eu1 Si1 O1 0.0 7_766 . . . ?
Si1 Eu1 Si1 O1 0.0 5_676 . . . ?
O4 Eu1 Si1 O2 -41.09(10) 3_465 . . . ?
O4 Eu1 Si1 O2 138.91(10) 7_766 . . . ?
O4 Eu1 Si1 O2 41.09(10) 8_576 . . . ?
O4 Eu1 Si1 O2 -138.91(10) 4_655 . . . ?
O1 Eu1 Si1 O2 180.0 . . . . ?
O1 Eu1 Si1 O2 0.0 5_676 . . . ?
Eu2 Eu1 Si1 O2 0.0 3_465 . . . ?
Na2 Eu1 Si1 O2 0.0 3_465 . . . ?
Na2 Eu1 Si1 O2 180.0 7_766 . . . ?
Eu2 Eu1 Si1 O2 180.0 7_766 . . . ?
Si1 Eu1 Si1 O2 180(100) 5_676 . . . ?
O4 Eu1 Si1 O3 -150.1(2) 3_465 . . 6_556 ?
O4 Eu1 Si1 O3 29.9(2) 7_766 . . 6_556 ?
O4 Eu1 Si1 O3 -67.9(2) 8_576 . . 6_556 ?
O4 Eu1 Si1 O3 112.1(2) 4_655 . . 6_556 ?
O1 Eu1 Si1 O3 71.0(2) . . . 6_556 ?
O1 Eu1 Si1 O3 -109.0(2) 5_676 . . 6_556 ?
Eu2 Eu1 Si1 O3 -109.0(2) 3_465 . . 6_556 ?
Na2 Eu1 Si1 O3 -109.0(2) 3_465 . . 6_556 ?
Na2 Eu1 Si1 O3 71.0(2) 7_766 . . 6_556 ?
Eu2 Eu1 Si1 O3 71.0(2) 7_766 . . 6_556 ?
Si1 Eu1 Si1 O3 71(100) 5_676 . . 6_556 ?
O4 Eu1 Si1 O3 67.9(2) 3_465 . . . ?
O4 Eu1 Si1 O3 -112.1(2) 7_766 . . . ?
O4 Eu1 Si1 O3 150.1(2) 8_576 . . . ?
O4 Eu1 Si1 O3 -29.9(2) 4_655 . . . ?
O1 Eu1 Si1 O3 -71.0(2) . . . . ?
O1 Eu1 Si1 O3 109.0(2) 5_676 . . . ?
Eu2 Eu1 Si1 O3 109.0(2) 3_465 . . . ?
Na2 Eu1 Si1 O3 109.0(2) 3_465 . . . ?
Na2 Eu1 Si1 O3 -71.0(2) 7_766 . . . ?
Eu2 Eu1 Si1 O3 -71.0(2) 7_766 . . . ?
Si1 Eu1 Si1 O3 -71(100) 5_676 . . . ?
O4 Eu1 Si1 Na1 -41.09(10) 3_465 . . 3_565 ?
O4 Eu1 Si1 Na1 138.91(10) 7_766 . . 3_565 ?
O4 Eu1 Si1 Na1 41.09(10) 8_576 . . 3_565 ?
O4 Eu1 Si1 Na1 -138.91(10) 4_655 . . 3_565 ?
O1 Eu1 Si1 Na1 180.0 . . . 3_565 ?
O1 Eu1 Si1 Na1 0.0 5_676 . . 3_565 ?
Eu2 Eu1 Si1 Na1 0.0 3_465 . . 3_565 ?
Na2 Eu1 Si1 Na1 0.0 3_465 . . 3_565 ?
Na2 Eu1 Si1 Na1 180.0 7_766 . . 3_565 ?
Eu2 Eu1 Si1 Na1 180.0 7_766 . . 3_565 ?
Si1 Eu1 Si1 Na1 180.0 5_676 . . 3_565 ?
O4 Eu1 Si1 Na4 16.62(12) 3_465 . . . ?
O4 Eu1 Si1 Na4 -163.38(12) 7_766 . . . ?
O4 Eu1 Si1 Na4 98.80(12) 8_576 . . . ?
O4 Eu1 Si1 Na4 -81.20(12) 4_655 . . . ?
O1 Eu1 Si1 Na4 -122.29(6) . . . . ?
O1 Eu1 Si1 Na4 57.71(6) 5_676 . . . ?
Eu2 Eu1 Si1 Na4 57.71(6) 3_465 . . . ?
Na2 Eu1 Si1 Na4 57.71(6) 3_465 . . . ?
Na2 Eu1 Si1 Na4 -122.29(6) 7_766 . . . ?
Eu2 Eu1 Si1 Na4 -122.29(6) 7_766 . . . ?
Si1 Eu1 Si1 Na4 -122(100) 5_676 . . . ?
O4 Eu1 Si1 Na4 -98.80(12) 3_465 . . 6_556 ?
O4 Eu1 Si1 Na4 81.20(12) 7_766 . . 6_556 ?
O4 Eu1 Si1 Na4 -16.62(12) 8_576 . . 6_556 ?
O4 Eu1 Si1 Na4 163.38(12) 4_655 . . 6_556 ?
O1 Eu1 Si1 Na4 122.29(6) . . . 6_556 ?
O1 Eu1 Si1 Na4 -57.71(6) 5_676 . . 6_556 ?
Eu2 Eu1 Si1 Na4 -57.71(6) 3_465 . . 6_556 ?
Na2 Eu1 Si1 Na4 -57.71(6) 3_465 . . 6_556 ?
Na2 Eu1 Si1 Na4 122.29(6) 7_766 . . 6_556 ?
Eu2 Eu1 Si1 Na4 122.29(6) 7_766 . . 6_556 ?
Si1 Eu1 Si1 Na4 122(100) 5_676 . . 6_556 ?
O4 Eu1 Si1 Na4 -160.39(12) 3_465 . . 7_766 ?
O4 Eu1 Si1 Na4 19.61(12) 7_766 . . 7_766 ?
O4 Eu1 Si1 Na4 -78.21(11) 8_576 . . 7_766 ?
O4 Eu1 Si1 Na4 101.79(11) 4_655 . . 7_766 ?
O1 Eu1 Si1 Na4 60.70(5) . . . 7_766 ?
O1 Eu1 Si1 Na4 -119.30(5) 5_676 . . 7_766 ?
Eu2 Eu1 Si1 Na4 -119.30(5) 3_465 . . 7_766 ?
Na2 Eu1 Si1 Na4 -119.30(5) 3_465 . . 7_766 ?
Na2 Eu1 Si1 Na4 60.70(5) 7_766 . . 7_766 ?
Eu2 Eu1 Si1 Na4 60.70(5) 7_766 . . 7_766 ?
Si1 Eu1 Si1 Na4 61(100) 5_676 . . 7_766 ?
O4 Eu1 Si1 Na4 78.21(11) 3_465 . . 4_655 ?
O4 Eu1 Si1 Na4 -101.79(11) 7_766 . . 4_655 ?
O4 Eu1 Si1 Na4 160.39(12) 8_576 . . 4_655 ?
O4 Eu1 Si1 Na4 -19.61(12) 4_655 . . 4_655 ?
O1 Eu1 Si1 Na4 -60.70(5) . . . 4_655 ?
O1 Eu1 Si1 Na4 119.30(5) 5_676 . . 4_655 ?
Eu2 Eu1 Si1 Na4 119.30(5) 3_465 . . 4_655 ?
Na2 Eu1 Si1 Na4 119.30(5) 3_465 . . 4_655 ?
Na2 Eu1 Si1 Na4 -60.70(5) 7_766 . . 4_655 ?
Eu2 Eu1 Si1 Na4 -60.70(5) 7_766 . . 4_655 ?
Si1 Eu1 Si1 Na4 -61(100) 5_676 . . 4_655 ?
O4 Eu1 Si1 Eu3 -41.09(10) 3_465 . . 3_465 ?
O4 Eu1 Si1 Eu3 138.91(10) 7_766 . . 3_465 ?
O4 Eu1 Si1 Eu3 41.09(10) 8_576 . . 3_465 ?
O4 Eu1 Si1 Eu3 -138.91(10) 4_655 . . 3_465 ?
O1 Eu1 Si1 Eu3 180.0 . . . 3_465 ?
O1 Eu1 Si1 Eu3 0.0 5_676 . . 3_465 ?
Eu2 Eu1 Si1 Eu3 0.0 3_465 . . 3_465 ?
Na2 Eu1 Si1 Eu3 0.0 3_465 . . 3_465 ?
Na2 Eu1 Si1 Eu3 180.0 7_766 . . 3_465 ?
Eu2 Eu1 Si1 Eu3 180.0 7_766 . . 3_465 ?
Si1 Eu1 Si1 Eu3 180.0 5_676 . . 3_465 ?
O6 Na4 Si2 O6 1.30(18) 2_765 . . . ?
O3 Na4 Si2 O6 95.2(3) . . . . ?
O6 Na4 Si2 O6 177.96(15) 3_465 . . . ?
O4 Na4 Si2 O6 -105.5(3) . . . . ?
O1 Na4 Si2 O6 -94.3(3) 7_755 . . . ?
O2 Na4 Si2 O6 85.3(2) . . . . ?
O5 Na4 Si2 O6 156.2(4) 3_465 . . . ?
O3 Na4 Si2 O6 -77.4(4) 4_645 . . . ?
Eu2 Na4 Si2 O6 -137.9(2) . . . . ?
Si1 Na4 Si2 O6 96.5(2) . . . . ?
O6 Na4 Si2 O4 106.8(2) 2_765 . . . ?
O3 Na4 Si2 O4 -159.3(3) . . . . ?
O6 Na4 Si2 O4 -76.6(2) 3_465 . . . ?
O1 Na4 Si2 O4 11.1(2) 7_755 . . . ?
O2 Na4 Si2 O4 -169.3(2) . . . . ?
O5 Na4 Si2 O4 -98.3(4) 3_465 . . . ?
O3 Na4 Si2 O4 28.1(3) 4_645 . . . ?
Eu2 Na4 Si2 O4 -32.42(18) . . . . ?
Si1 Na4 Si2 O4 -158.0(2) . . . . ?
O6 Na4 Si2 O5 -172.4(4) 2_765 . . . ?
O3 Na4 Si2 O5 -78.4(5) . . . . ?
O6 Na4 Si2 O5 4.3(5) 3_465 . . . ?
O4 Na4 Si2 O5 80.9(5) . . . . ?
O1 Na4 Si2 O5 92.0(4) 7_755 . . . ?
O2 Na4 Si2 O5 -88.4(5) . . . . ?
O5 Na4 Si2 O5 -17.4(8) 3_465 . . . ?
O3 Na4 Si2 O5 109.0(5) 4_645 . . . ?
Eu2 Na4 Si2 O5 48.5(4) . . . . ?
Si1 Na4 Si2 O5 -77.1(4) . . . . ?
O6 Na4 Si2 O3 -93.9(3) 2_765 . . . ?
O6 Na4 Si2 O3 82.7(3) 3_465 . . . ?
O4 Na4 Si2 O3 159.3(3) . . . . ?
O1 Na4 Si2 O3 170.5(3) 7_755 . . . ?
O2 Na4 Si2 O3 -9.9(3) . . . . ?
O5 Na4 Si2 O3 61.0(5) 3_465 . . . ?
O3 Na4 Si2 O3 -172.6(4) 4_645 . . . ?
Eu2 Na4 Si2 O3 126.9(3) . . . . ?
Si1 Na4 Si2 O3 1.3(3) . . . . ?
O6 Na4 Si2 Na1 -34.10(13) 2_765 . . 3_565 ?
O3 Na4 Si2 Na1 59.8(3) . . . 3_565 ?
O6 Na4 Si2 Na1 142.57(12) 3_465 . . 3_565 ?
O4 Na4 Si2 Na1 -140.8(2) . . . 3_565 ?
O1 Na4 Si2 Na1 -129.70(14) 7_755 . . 3_565 ?
O2 Na4 Si2 Na1 49.89(12) . . . 3_565 ?
O5 Na4 Si2 Na1 120.8(4) 3_465 . . 3_565 ?
O3 Na4 Si2 Na1 -112.7(3) 4_645 . . 3_565 ?
Eu2 Na4 Si2 Na1 -173.27(6) . . . 3_565 ?
Si1 Na4 Si2 Na1 61.12(5) . . . 3_565 ?
O6 Na4 Si2 Na4 58.7(3) 2_765 . . 3_565 ?
O3 Na4 Si2 Na4 152.6(4) . . . 3_565 ?
O6 Na4 Si2 Na4 -124.6(3) 3_465 . . 3_565 ?
O4 Na4 Si2 Na4 -48.0(3) . . . 3_565 ?
O1 Na4 Si2 Na4 -36.9(3) 7_755 . . 3_565 ?
O2 Na4 Si2 Na4 142.7(3) . . . 3_565 ?
O5 Na4 Si2 Na4 -146.4(4) 3_465 . . 3_565 ?
O3 Na4 Si2 Na4 -19.9(4) 4_645 . . 3_565 ?
Eu2 Na4 Si2 Na4 -80.5(3) . . . 3_565 ?
Si1 Na4 Si2 Na4 153.9(3) . . . 3_565 ?
O6 Na4 Si2 Na4 -162.59(18) 2_765 . . 4_655 ?
O3 Na4 Si2 Na4 -68.7(3) . . . 4_655 ?
O6 Na4 Si2 Na4 14.07(10) 3_465 . . 4_655 ?
O4 Na4 Si2 Na4 90.7(2) . . . 4_655 ?
O1 Na4 Si2 Na4 101.81(16) 7_755 . . 4_655 ?
O2 Na4 Si2 Na4 -78.60(14) . . . 4_655 ?
O5 Na4 Si2 Na4 -7.7(4) 3_465 . . 4_655 ?
O3 Na4 Si2 Na4 118.8(3) 4_645 . . 4_655 ?
Eu2 Na4 Si2 Na4 58.24(6) . . . 4_655 ?
Si1 Na4 Si2 Na4 -67.38(8) . . . 4_655 ?
O6 Na4 Si2 Eu3 132.23(14) 2_765 . . . ?
O3 Na4 Si2 Eu3 -133.8(3) . . . . ?
O6 Na4 Si2 Eu3 -51.11(12) 3_465 . . . ?
O4 Na4 Si2 Eu3 25.48(18) . . . . ?
O1 Na4 Si2 Eu3 36.63(14) 7_755 . . . ?
O2 Na4 Si2 Eu3 -143.78(13) . . . . ?
O5 Na4 Si2 Eu3 -72.9(4) 3_465 . . . ?
O3 Na4 Si2 Eu3 53.6(3) 4_645 . . . ?
Eu2 Na4 Si2 Eu3 -6.94(5) . . . . ?
Si1 Na4 Si2 Eu3 -132.56(7) . . . . ?
O6 Na4 Si2 Eu1 78.19(13) 2_765 . . 3_565 ?
O3 Na4 Si2 Eu1 172.1(3) . . . 3_565 ?
O6 Na4 Si2 Eu1 -105.15(12) 3_465 . . 3_565 ?
O4 Na4 Si2 Eu1 -28.57(18) . . . 3_565 ?
O1 Na4 Si2 Eu1 -17.42(13) 7_755 . . 3_565 ?
O2 Na4 Si2 Eu1 162.18(14) . . . 3_565 ?
O5 Na4 Si2 Eu1 -126.9(4) 3_465 . . 3_565 ?
O3 Na4 Si2 Eu1 -0.5(3) 4_645 . . 3_565 ?
Eu2 Na4 Si2 Eu1 -60.99(4) . . . 3_565 ?
Si1 Na4 Si2 Eu1 173.40(7) . . . 3_565 ?
O6 Na4 Si2 Eu2 -25.95(16) 2_765 . . 3_565 ?
O3 Na4 Si2 Eu2 68.0(3) . . . 3_565 ?
O6 Na4 Si2 Eu2 150.72(12) 3_465 . . 3_565 ?
O4 Na4 Si2 Eu2 -132.7(2) . . . 3_565 ?
O1 Na4 Si2 Eu2 -121.55(15) 7_755 . . 3_565 ?
O2 Na4 Si2 Eu2 58.04(14) . . . 3_565 ?
O5 Na4 Si2 Eu2 129.0(4) 3_465 . . 3_565 ?
O3 Na4 Si2 Eu2 -104.6(3) 4_645 . . 3_565 ?
Eu2 Na4 Si2 Eu2 -165.12(7) . . . 3_565 ?
Si1 Na4 Si2 Eu2 69.27(8) . . . 3_565 ?
O2 Eu3 Si2 O6 2.6(2) 3_565 . . . ?
O2 Eu3 Si2 O6 -177.4(2) 7_765 . . . ?
O4 Eu3 Si2 O6 93.1(2) 6 . . . ?
O4 Eu3 Si2 O6 -86.9(2) 2_775 . . . ?
O4 Eu3 Si2 O6 105.4(3) . . . . ?
O4 Eu3 Si2 O6 -74.6(3) 5_775 . . . ?
O5 Eu3 Si2 O6 82.1(2) 5_775 . . . ?
O5 Eu3 Si2 O6 -97.9(2) . . . . ?
Eu2 Eu3 Si2 O6 138.8(2) . . . . ?
Eu2 Eu3 Si2 O6 -41.2(2) 5_775 . . . ?
Si2 Eu3 Si2 O6 82.1(2) 6 . . . ?
Si2 Eu3 Si2 O6 -97.9(2) 2_775 . . . ?
O2 Eu3 Si2 O4 -102.8(2) 3_565 . . . ?
O2 Eu3 Si2 O4 77.2(2) 7_765 . . . ?
O4 Eu3 Si2 O4 -12.37(12) 6 . . . ?
O4 Eu3 Si2 O4 167.63(12) 2_775 . . . ?
O4 Eu3 Si2 O4 180.0 5_775 . . . ?
O5 Eu3 Si2 O4 -23.3(2) 5_775 . . . ?
O5 Eu3 Si2 O4 156.7(2) . . . . ?
Eu2 Eu3 Si2 O4 33.34(19) . . . . ?
Eu2 Eu3 Si2 O4 -146.66(19) 5_775 . . . ?
Si2 Eu3 Si2 O4 -23.3(2) 6 . . . ?
Si2 Eu3 Si2 O4 156.7(2) 2_775 . . . ?
O2 Eu3 Si2 O5 100.50(13) 3_565 . . . ?
O2 Eu3 Si2 O5 -79.50(13) 7_765 . . . ?
O4 Eu3 Si2 O5 -169.07(10) 6 . . . ?
O4 Eu3 Si2 O5 10.93(10) 2_775 . . . ?
O4 Eu3 Si2 O5 -156.7(2) . . . . ?
O4 Eu3 Si2 O5 23.3(2) 5_775 . . . ?
O5 Eu3 Si2 O5 180.000(1) 5_775 . . . ?
Eu2 Eu3 Si2 O5 -123.36(5) . . . . ?
Eu2 Eu3 Si2 O5 56.64(5) 5_775 . . . ?
Si2 Eu3 Si2 O5 180.000(1) 6 . . . ?
Si2 Eu3 Si2 O5 0.000(1) 2_775 . . . ?
O2 Eu3 Si2 O3 -180.0(3) 3_565 . . . ?
O2 Eu3 Si2 O3 0.0(3) 7_765 . . . ?
O4 Eu3 Si2 O3 -89.5(3) 6 . . . ?
O4 Eu3 Si2 O3 90.5(3) 2_775 . . . ?
O4 Eu3 Si2 O3 -77.2(3) . . . . ?
O4 Eu3 Si2 O3 102.8(3) 5_775 . . . ?
O5 Eu3 Si2 O3 -100.5(2) 5_775 . . . ?
O5 Eu3 Si2 O3 79.5(2) . . . . ?
Eu2 Eu3 Si2 O3 -43.8(2) . . . . ?
Eu2 Eu3 Si2 O3 136.2(2) 5_775 . . . ?
Si2 Eu3 Si2 O3 -100.5(2) 6 . . . ?
Si2 Eu3 Si2 O3 79.5(2) 2_775 . . . ?
O2 Eu3 Si2 Na4 -129.16(13) 3_565 . . . ?
O2 Eu3 Si2 Na4 50.84(13) 7_765 . . . ?
O4 Eu3 Si2 Na4 -38.73(11) 6 . . . ?
O4 Eu3 Si2 Na4 141.27(11) 2_775 . . . ?
O4 Eu3 Si2 Na4 -26.36(19) . . . . ?
O4 Eu3 Si2 Na4 153.64(19) 5_775 . . . ?
O5 Eu3 Si2 Na4 -49.66(8) 5_775 . . . ?
O5 Eu3 Si2 Na4 130.34(8) . . . . ?
Eu2 Eu3 Si2 Na4 6.98(5) . . . . ?
Eu2 Eu3 Si2 Na4 -173.02(5) 5_775 . . . ?
Si2 Eu3 Si2 Na4 -49.66(8) 6 . . . ?
Si2 Eu3 Si2 Na4 130.34(8) 2_775 . . . ?
O2 Eu3 Si2 Na1 -62.8(2) 3_565 . . 3_565 ?
O2 Eu3 Si2 Na1 117.2(2) 7_765 . . 3_565 ?
O4 Eu3 Si2 Na1 27.7(2) 6 . . 3_565 ?
O4 Eu3 Si2 Na1 -152.3(2) 2_775 . . 3_565 ?
O4 Eu3 Si2 Na1 40.0(2) . . . 3_565 ?
O4 Eu3 Si2 Na1 -140.0(2) 5_775 . . 3_565 ?
O5 Eu3 Si2 Na1 16.7(2) 5_775 . . 3_565 ?
O5 Eu3 Si2 Na1 -163.3(2) . . . 3_565 ?
Eu2 Eu3 Si2 Na1 73.37(18) . . . 3_565 ?
Eu2 Eu3 Si2 Na1 -106.63(18) 5_775 . . 3_565 ?
Si2 Eu3 Si2 Na1 16.7(2) 6 . . 3_565 ?
Si2 Eu3 Si2 Na1 -163.3(2) 2_775 . . 3_565 ?
O2 Eu3 Si2 Na4 34.77(14) 3_565 . . 3_565 ?
O2 Eu3 Si2 Na4 -145.23(14) 7_765 . . 3_565 ?
O4 Eu3 Si2 Na4 125.20(11) 6 . . 3_565 ?
O4 Eu3 Si2 Na4 -54.80(11) 2_775 . . 3_565 ?
O4 Eu3 Si2 Na4 137.6(2) . . . 3_565 ?
O4 Eu3 Si2 Na4 -42.4(2) 5_775 . . 3_565 ?
O5 Eu3 Si2 Na4 114.27(6) 5_775 . . 3_565 ?
O5 Eu3 Si2 Na4 -65.73(6) . . . 3_565 ?
Eu2 Eu3 Si2 Na4 170.91(7) . . . 3_565 ?
Eu2 Eu3 Si2 Na4 -9.09(7) 5_775 . . 3_565 ?
Si2 Eu3 Si2 Na4 114.27(6) 6 . . 3_565 ?
Si2 Eu3 Si2 Na4 -65.73(6) 2_775 . . 3_565 ?
O2 Eu3 Si2 Na4 165.60(13) 3_565 . . 4_655 ?
O2 Eu3 Si2 Na4 -14.40(13) 7_765 . . 4_655 ?
O4 Eu3 Si2 Na4 -103.97(10) 6 . . 4_655 ?
O4 Eu3 Si2 Na4 76.03(10) 2_775 . . 4_655 ?
O4 Eu3 Si2 Na4 -91.6(2) . . . 4_655 ?
O4 Eu3 Si2 Na4 88.4(2) 5_775 . . 4_655 ?
O5 Eu3 Si2 Na4 -114.91(6) 5_775 . . 4_655 ?
O5 Eu3 Si2 Na4 65.09(6) . . . 4_655 ?
Eu2 Eu3 Si2 Na4 -58.26(5) . . . 4_655 ?
Eu2 Eu3 Si2 Na4 121.74(5) 5_775 . . 4_655 ?
Si2 Eu3 Si2 Na4 -114.91(6) 6 . . 4_655 ?
Si2 Eu3 Si2 Na4 65.09(6) 2_775 . . 4_655 ?
O2 Eu3 Si2 Eu1 -75.60(12) 3_565 . . 3_565 ?
O2 Eu3 Si2 Eu1 104.40(12) 7_765 . . 3_565 ?
O4 Eu3 Si2 Eu1 14.83(9) 6 . . 3_565 ?
O4 Eu3 Si2 Eu1 -165.17(9) 2_775 . . 3_565 ?
O4 Eu3 Si2 Eu1 27.20(19) . . . 3_565 ?
O4 Eu3 Si2 Eu1 -152.80(19) 5_775 . . 3_565 ?
O5 Eu3 Si2 Eu1 3.89(5) 5_775 . . 3_565 ?
O5 Eu3 Si2 Eu1 -176.11(5) . . . 3_565 ?
Eu2 Eu3 Si2 Eu1 60.54(3) . . . 3_565 ?
Eu2 Eu3 Si2 Eu1 -119.46(3) 5_775 . . 3_565 ?
Si2 Eu3 Si2 Eu1 3.89(5) 6 . . 3_565 ?
Si2 Eu3 Si2 Eu1 -176.11(5) 2_775 . . 3_565 ?
O2 Eu3 Si2 Eu2 28.91(14) 3_565 . . 3_565 ?
O2 Eu3 Si2 Eu2 -151.09(14) 7_765 . . 3_565 ?
O4 Eu3 Si2 Eu2 119.34(11) 6 . . 3_565 ?
O4 Eu3 Si2 Eu2 -60.66(11) 2_775 . . 3_565 ?
O4 Eu3 Si2 Eu2 131.7(2) . . . 3_565 ?
O4 Eu3 Si2 Eu2 -48.3(2) 5_775 . . 3_565 ?
O5 Eu3 Si2 Eu2 108.41(6) 5_775 . . 3_565 ?
O5 Eu3 Si2 Eu2 -71.59(6) . . . 3_565 ?
Eu2 Eu3 Si2 Eu2 165.05(7) . . . 3_565 ?
Eu2 Eu3 Si2 Eu2 -14.95(7) 5_775 . . 3_565 ?
Si2 Eu3 Si2 Eu2 108.41(6) 6 . . 3_565 ?
Si2 Eu3 Si2 Eu2 -71.59(6) 2_775 . . 3_565 ?
O2 Si1 O1 Eu1 0.0 . . . . ?
O3 Si1 O1 Eu1 -122.5(2) 6_556 . . . ?
O3 Si1 O1 Eu1 122.5(2) . . . . ?
Na1 Si1 O1 Eu1 180.0 3_565 . . . ?
Na4 Si1 O1 Eu1 66.46(12) . . . . ?
Na4 Si1 O1 Eu1 -66.46(12) 6_556 . . . ?
Na4 Si1 O1 Eu1 -102.64(16) 7_766 . . . ?
Na4 Si1 O1 Eu1 102.64(16) 4_655 . . . ?
Eu3 Si1 O1 Eu1 0.0 3_465 . . . ?
O2 Si1 O1 Na2 180.0 . . . 7_766 ?
O3 Si1 O1 Na2 57.5(2) 6_556 . . 7_766 ?
O3 Si1 O1 Na2 -57.5(2) . . . 7_766 ?
Na1 Si1 O1 Na2 0.0 3_565 . . 7_766 ?
Na4 Si1 O1 Na2 -113.54(12) . . . 7_766 ?
Na4 Si1 O1 Na2 113.54(12) 6_556 . . 7_766 ?
Na4 Si1 O1 Na2 77.36(16) 7_766 . . 7_766 ?
Na4 Si1 O1 Na2 -77.36(16) 4_655 . . 7_766 ?
Eu1 Si1 O1 Na2 180.0 . . . 7_766 ?
Eu3 Si1 O1 Na2 180.0 3_465 . . 7_766 ?
O2 Si1 O1 Eu2 180.0 . . . 7_766 ?
O3 Si1 O1 Eu2 57.5(2) 6_556 . . 7_766 ?
O3 Si1 O1 Eu2 -57.5(2) . . . 7_766 ?
Na1 Si1 O1 Eu2 0.0 3_565 . . 7_766 ?
Na4 Si1 O1 Eu2 -113.54(12) . . . 7_766 ?
Na4 Si1 O1 Eu2 113.54(12) 6_556 . . 7_766 ?
Na4 Si1 O1 Eu2 77.36(16) 7_766 . . 7_766 ?
Na4 Si1 O1 Eu2 -77.36(16) 4_655 . . 7_766 ?
Eu1 Si1 O1 Eu2 180.0 . . . 7_766 ?
Eu3 Si1 O1 Eu2 180.0 3_465 . . 7_766 ?
O2 Si1 O1 Na4 102.64(16) . . . 7_766 ?
O3 Si1 O1 Na4 -19.9(3) 6_556 . . 7_766 ?
O3 Si1 O1 Na4 -134.9(2) . . . 7_766 ?
Na1 Si1 O1 Na4 -77.36(16) 3_565 . . 7_766 ?
Na4 Si1 O1 Na4 169.10(10) . . . 7_766 ?
Na4 Si1 O1 Na4 36.2(3) 6_556 . . 7_766 ?
Na4 Si1 O1 Na4 -154.7(3) 4_655 . . 7_766 ?
Eu1 Si1 O1 Na4 102.64(16) . . . 7_766 ?
Eu3 Si1 O1 Na4 102.64(16) 3_465 . . 7_766 ?
O2 Si1 O1 Na4 -102.64(16) . . . 4_655 ?
O3 Si1 O1 Na4 134.9(2) 6_556 . . 4_655 ?
O3 Si1 O1 Na4 19.9(3) . . . 4_655 ?
Na1 Si1 O1 Na4 77.36(16) 3_565 . . 4_655 ?
Na4 Si1 O1 Na4 -36.2(3) . . . 4_655 ?
Na4 Si1 O1 Na4 -169.10(10) 6_556 . . 4_655 ?
Na4 Si1 O1 Na4 154.7(3) 7_766 . . 4_655 ?
Eu1 Si1 O1 Na4 -102.64(16) . . . 4_655 ?
Eu3 Si1 O1 Na4 -102.64(16) 3_465 . . 4_655 ?
O4 Eu1 O1 Si1 -41.21(11) 3_465 . . . ?
O4 Eu1 O1 Si1 138.79(11) 7_766 . . . ?
O4 Eu1 O1 Si1 41.21(11) 8_576 . . . ?
O4 Eu1 O1 Si1 -138.79(11) 4_655 . . . ?
O1 Eu1 O1 Si1 180(100) 5_676 . . . ?
Eu2 Eu1 O1 Si1 0.0 3_465 . . . ?
Na2 Eu1 O1 Si1 0.0 3_465 . . . ?
Na2 Eu1 O1 Si1 180.0 7_766 . . . ?
Eu2 Eu1 O1 Si1 180.0 7_766 . . . ?
Si1 Eu1 O1 Si1 180.0 5_676 . . . ?
O4 Eu1 O1 Na2 138.79(11) 3_465 . . 7_766 ?
O4 Eu1 O1 Na2 -41.21(11) 7_766 . . 7_766 ?
O4 Eu1 O1 Na2 -138.79(11) 8_576 . . 7_766 ?
O4 Eu1 O1 Na2 41.21(11) 4_655 . . 7_766 ?
O1 Eu1 O1 Na2 0.0 5_676 . . 7_766 ?
Eu2 Eu1 O1 Na2 180.0 3_465 . . 7_766 ?
Na2 Eu1 O1 Na2 180.0 3_465 . . 7_766 ?
Eu2 Eu1 O1 Na2 0.0 7_766 . . 7_766 ?
Si1 Eu1 O1 Na2 180.0 . . . 7_766 ?
Si1 Eu1 O1 Na2 0.0 5_676 . . 7_766 ?
O4 Eu1 O1 Eu2 138.79(11) 3_465 . . 7_766 ?
O4 Eu1 O1 Eu2 -41.21(11) 7_766 . . 7_766 ?
O4 Eu1 O1 Eu2 -138.79(11) 8_576 . . 7_766 ?
O4 Eu1 O1 Eu2 41.21(11) 4_655 . . 7_766 ?
O1 Eu1 O1 Eu2 0.0 5_676 . . 7_766 ?
Eu2 Eu1 O1 Eu2 180.0 3_465 . . 7_766 ?
Na2 Eu1 O1 Eu2 180.0 3_465 . . 7_766 ?
Na2 Eu1 O1 Eu2 0.0 7_766 . . 7_766 ?
Si1 Eu1 O1 Eu2 180.0 . . . 7_766 ?
Si1 Eu1 O1 Eu2 0.0 5_676 . . 7_766 ?
O4 Eu1 O1 Na4 -145.84(17) 3_465 . . 7_766 ?
O4 Eu1 O1 Na4 34.16(17) 7_766 . . 7_766 ?
O4 Eu1 O1 Na4 -63.42(18) 8_576 . . 7_766 ?
O4 Eu1 O1 Na4 116.58(18) 4_655 . . 7_766 ?
O1 Eu1 O1 Na4 75(100) 5_676 . . 7_766 ?
Eu2 Eu1 O1 Na4 -104.63(14) 3_465 . . 7_766 ?
Na2 Eu1 O1 Na4 -104.63(14) 3_465 . . 7_766 ?
Na2 Eu1 O1 Na4 75.37(14) 7_766 . . 7_766 ?
Eu2 Eu1 O1 Na4 75.37(14) 7_766 . . 7_766 ?
Si1 Eu1 O1 Na4 -104.63(14) . . . 7_766 ?
Si1 Eu1 O1 Na4 75.37(14) 5_676 . . 7_766 ?
O4 Eu1 O1 Na4 63.42(18) 3_465 . . 4_655 ?
O4 Eu1 O1 Na4 -116.58(18) 7_766 . . 4_655 ?
O4 Eu1 O1 Na4 145.84(17) 8_576 . . 4_655 ?
O4 Eu1 O1 Na4 -34.16(17) 4_655 . . 4_655 ?
O1 Eu1 O1 Na4 -75(100) 5_676 . . 4_655 ?
Eu2 Eu1 O1 Na4 104.63(14) 3_465 . . 4_655 ?
Na2 Eu1 O1 Na4 104.63(14) 3_465 . . 4_655 ?
Na2 Eu1 O1 Na4 -75.37(14) 7_766 . . 4_655 ?
Eu2 Eu1 O1 Na4 -75.37(14) 7_766 . . 4_655 ?
Si1 Eu1 O1 Na4 104.63(14) . . . 4_655 ?
Si1 Eu1 O1 Na4 -75.37(14) 5_676 . . 4_655 ?
O1 Si1 O2 Na3 0.0 . . . 3_465 ?
O3 Si1 O2 Na3 124.5(2) 6_556 . . 3_465 ?
O3 Si1 O2 Na3 -124.5(2) . . . 3_465 ?
Na1 Si1 O2 Na3 180.0 3_565 . . 3_465 ?
Na4 Si1 O2 Na3 -104.83(13) . . . 3_465 ?
Na4 Si1 O2 Na3 104.83(13) 6_556 . . 3_465 ?
Na4 Si1 O2 Na3 60.17(12) 7_766 . . 3_465 ?
Na4 Si1 O2 Na3 -60.17(12) 4_655 . . 3_465 ?
Eu1 Si1 O2 Na3 0.0 . . . 3_465 ?
Eu3 Si1 O2 Na3 0.0 3_465 . . 3_465 ?
O1 Si1 O2 Eu3 0.0 . . . 3_465 ?
O3 Si1 O2 Eu3 124.5(2) 6_556 . . 3_465 ?
O3 Si1 O2 Eu3 -124.5(2) . . . 3_465 ?
Na1 Si1 O2 Eu3 180.0 3_565 . . 3_465 ?
Na4 Si1 O2 Eu3 -104.83(13) . . . 3_465 ?
Na4 Si1 O2 Eu3 104.83(13) 6_556 . . 3_465 ?
Na4 Si1 O2 Eu3 60.17(12) 7_766 . . 3_465 ?
Na4 Si1 O2 Eu3 -60.17(12) 4_655 . . 3_465 ?
Eu1 Si1 O2 Eu3 0.0 . . . 3_465 ?
O1 Si1 O2 Na2 180.0 . . . 7_756 ?
O3 Si1 O2 Na2 -55.5(2) 6_556 . . 7_756 ?
O3 Si1 O2 Na2 55.5(2) . . . 7_756 ?
Na1 Si1 O2 Na2 0.0 3_565 . . 7_756 ?
Na4 Si1 O2 Na2 75.17(13) . . . 7_756 ?
Na4 Si1 O2 Na2 -75.17(13) 6_556 . . 7_756 ?
Na4 Si1 O2 Na2 -119.83(12) 7_766 . . 7_756 ?
Na4 Si1 O2 Na2 119.83(12) 4_655 . . 7_756 ?
Eu1 Si1 O2 Na2 180.0 . . . 7_756 ?
Eu3 Si1 O2 Na2 180.0 3_465 . . 7_756 ?
O1 Si1 O2 Eu2 180.0 . . . 7_756 ?
O3 Si1 O2 Eu2 -55.5(2) 6_556 . . 7_756 ?
O3 Si1 O2 Eu2 55.5(2) . . . 7_756 ?
Na1 Si1 O2 Eu2 0.0 3_565 . . 7_756 ?
Na4 Si1 O2 Eu2 75.17(13) . . . 7_756 ?
Na4 Si1 O2 Eu2 -75.17(13) 6_556 . . 7_756 ?
Na4 Si1 O2 Eu2 -119.83(12) 7_766 . . 7_756 ?
Na4 Si1 O2 Eu2 119.83(12) 4_655 . . 7_756 ?
Eu1 Si1 O2 Eu2 180.0 . . . 7_756 ?
Eu3 Si1 O2 Eu2 180.0 3_465 . . 7_756 ?
O1 Si1 O2 Na4 -104.83(13) . . . 6_556 ?
O3 Si1 O2 Na4 19.7(3) 6_556 . . 6_556 ?
O3 Si1 O2 Na4 130.6(3) . . . 6_556 ?
Na1 Si1 O2 Na4 75.17(13) 3_565 . . 6_556 ?
Na4 Si1 O2 Na4 150.3(3) . . . 6_556 ?
Na4 Si1 O2 Na4 -44.7(2) 7_766 . . 6_556 ?
Na4 Si1 O2 Na4 -165.00(10) 4_655 . . 6_556 ?
Eu1 Si1 O2 Na4 -104.83(13) . . . 6_556 ?
Eu3 Si1 O2 Na4 -104.83(13) 3_465 . . 6_556 ?
O1 Si1 O2 Na4 104.83(13) . . . . ?
O3 Si1 O2 Na4 -130.6(3) 6_556 . . . ?
O3 Si1 O2 Na4 -19.7(3) . . . . ?
Na1 Si1 O2 Na4 -75.17(13) 3_565 . . . ?
Na4 Si1 O2 Na4 -150.3(3) 6_556 . . . ?
Na4 Si1 O2 Na4 165.00(10) 7_766 . . . ?
Na4 Si1 O2 Na4 44.7(2) 4_655 . . . ?
Eu1 Si1 O2 Na4 104.83(13) . . . . ?
Eu3 Si1 O2 Na4 104.83(13) 3_465 . . . ?
O6 Na4 O2 Si1 110.1(3) 2_765 . . . ?
O3 Na4 O2 Si1 14.0(2) . . . . ?
O6 Na4 O2 Si1 -70.5(2) 3_465 . . . ?
O4 Na4 O2 Si1 13.9(3) . . . . ?
O1 Na4 O2 Si1 -163.4(14) 7_755 . . . ?
O5 Na4 O2 Si1 -126.8(2) 3_465 . . . ?
O3 Na4 O2 Si1 -168.7(2) 4_645 . . . ?
Eu2 Na4 O2 Si1 -47.5(3) . . . . ?
Si2 Na4 O2 Si1 20.0(2) . . . . ?
O6 Na4 O2 Na3 -111.3(2) 2_765 . . 3_465 ?
O3 Na4 O2 Na3 152.6(3) . . . 3_465 ?
O6 Na4 O2 Na3 68.16(19) 3_465 . . 3_465 ?
O4 Na4 O2 Na3 152.50(17) . . . 3_465 ?
O1 Na4 O2 Na3 -24.7(16) 7_755 . . 3_465 ?
O5 Na4 O2 Na3 11.80(15) 3_465 . . 3_465 ?
O3 Na4 O2 Na3 -30.1(3) 4_645 . . 3_465 ?
Eu2 Na4 O2 Na3 91.2(2) . . . 3_465 ?
Si2 Na4 O2 Na3 158.58(17) . . . 3_465 ?
Si1 Na4 O2 Na3 138.6(3) . . . 3_465 ?
O6 Na4 O2 Eu3 -111.3(2) 2_765 . . 3_465 ?
O3 Na4 O2 Eu3 152.6(3) . . . 3_465 ?
O6 Na4 O2 Eu3 68.16(19) 3_465 . . 3_465 ?
O4 Na4 O2 Eu3 152.50(17) . . . 3_465 ?
O1 Na4 O2 Eu3 -24.7(16) 7_755 . . 3_465 ?
O5 Na4 O2 Eu3 11.80(15) 3_465 . . 3_465 ?
O3 Na4 O2 Eu3 -30.1(3) 4_645 . . 3_465 ?
Eu2 Na4 O2 Eu3 91.2(2) . . . 3_465 ?
Si2 Na4 O2 Eu3 158.58(17) . . . 3_465 ?
Si1 Na4 O2 Eu3 138.6(3) . . . 3_465 ?
O6 Na4 O2 Na2 -28.40(17) 2_765 . . 7_756 ?
O3 Na4 O2 Na2 -124.5(2) . . . 7_756 ?
O6 Na4 O2 Na2 151.04(16) 3_465 . . 7_756 ?
O4 Na4 O2 Na2 -124.62(17) . . . 7_756 ?
O1 Na4 O2 Na2 58.1(16) 7_755 . . 7_756 ?
O5 Na4 O2 Na2 94.67(13) 3_465 . . 7_756 ?
O3 Na4 O2 Na2 52.8(2) 4_645 . . 7_756 ?
Eu2 Na4 O2 Na2 174.03(14) . . . 7_756 ?
Si2 Na4 O2 Na2 -118.54(13) . . . 7_756 ?
Si1 Na4 O2 Na2 -138.5(3) . . . 7_756 ?
O6 Na4 O2 Eu2 -28.40(17) 2_765 . . 7_756 ?
O3 Na4 O2 Eu2 -124.5(2) . . . 7_756 ?
O6 Na4 O2 Eu2 151.04(16) 3_465 . . 7_756 ?
O4 Na4 O2 Eu2 -124.62(17) . . . 7_756 ?
O1 Na4 O2 Eu2 58.1(16) 7_755 . . 7_756 ?
O5 Na4 O2 Eu2 94.67(13) 3_465 . . 7_756 ?
O3 Na4 O2 Eu2 52.8(2) 4_645 . . 7_756 ?
Eu2 Na4 O2 Eu2 174.03(14) . . . 7_756 ?
Si2 Na4 O2 Eu2 -118.54(13) . . . 7_756 ?
Si1 Na4 O2 Eu2 -138.5(3) . . . 7_756 ?
O6 Na4 O2 Na4 15.1(5) 2_765 . . 6_556 ?
O3 Na4 O2 Na4 -81.0(5) . . . 6_556 ?
O6 Na4 O2 Na4 -165.5(4) 3_465 . . 6_556 ?
O4 Na4 O2 Na4 -81.1(5) . . . 6_556 ?
O1 Na4 O2 Na4 101.6(15) 7_755 . . 6_556 ?
O5 Na4 O2 Na4 138.1(5) 3_465 . . 6_556 ?
O3 Na4 O2 Na4 96.3(5) 4_645 . . 6_556 ?
Eu2 Na4 O2 Na4 -142.5(4) . . . 6_556 ?
Si2 Na4 O2 Na4 -75.1(5) . . . 6_556 ?
Si1 Na4 O2 Na4 -95.0(5) . . . 6_556 ?
O1 Si1 O3 Si2 65.2(16) . . . . ?
O2 Si1 O3 Si2 -166.5(15) . . . . ?
O3 Si1 O3 Si2 -53.8(17) 6_556 . . . ?
Na1 Si1 O3 Si2 -96.9(15) 3_565 . . . ?
Na4 Si1 O3 Si2 171.9(17) . . . . ?
Na4 Si1 O3 Si2 -103.7(15) 6_556 . . . ?
Na4 Si1 O3 Si2 7.2(18) 7_766 . . . ?
Na4 Si1 O3 Si2 83.5(15) 4_655 . . . ?
Eu1 Si1 O3 Si2 94.2(15) . . . . ?
Eu3 Si1 O3 Si2 169.6(14) 3_465 . . . ?
O1 Si1 O3 Na4 -106.7(3) . . . . ?
O2 Si1 O3 Na4 21.7(3) . . . . ?
O3 Si1 O3 Na4 134.33(18) 6_556 . . . ?
Na1 Si1 O3 Na4 91.28(19) 3_565 . . . ?
Na4 Si1 O3 Na4 84.4(3) 6_556 . . . ?
Na4 Si1 O3 Na4 -164.66(17) 7_766 . . . ?
Na4 Si1 O3 Na4 -88.3(2) 4_655 . . . ?
Eu1 Si1 O3 Na4 -77.6(2) . . . . ?
Eu3 Si1 O3 Na4 -2.3(3) 3_465 . . . ?
O1 Si1 O3 Na1 162.0(2) . . . 3_565 ?
O2 Si1 O3 Na1 -69.6(2) . . . 3_565 ?
O3 Si1 O3 Na1 43.0(3) 6_556 . . 3_565 ?
Na4 Si1 O3 Na1 -91.28(19) . . . 3_565 ?
Na4 Si1 O3 Na1 -6.9(3) 6_556 . . 3_565 ?
Na4 Si1 O3 Na1 104.1(3) 7_766 . . 3_565 ?
Na4 Si1 O3 Na1 -179.6(2) 4_655 . . 3_565 ?
Eu1 Si1 O3 Na1 -168.89(9) . . . 3_565 ?
Eu3 Si1 O3 Na1 -93.59(17) 3_465 . . 3_565 ?
O1 Si1 O3 Na4 -18.3(3) . . . 4_655 ?
O2 Si1 O3 Na4 110.0(2) . . . 4_655 ?
O3 Si1 O3 Na4 -137.3(2) 6_556 . . 4_655 ?
Na1 Si1 O3 Na4 179.6(2) 3_565 . . 4_655 ?
Na4 Si1 O3 Na4 88.3(2) . . . 4_655 ?
Na4 Si1 O3 Na4 172.74(15) 6_556 . . 4_655 ?
Na4 Si1 O3 Na4 -76.3(3) 7_766 . . 4_655 ?
Eu1 Si1 O3 Na4 10.7(2) . . . 4_655 ?
Eu3 Si1 O3 Na4 86.03(16) 3_465 . . 4_655 ?
O6 Si2 O3 Si1 78.0(16) . . . . ?
O4 Si2 O3 Si1 -154.1(15) . . . . ?
O5 Si2 O3 Si1 -42.5(16) . . . . ?
Na4 Si2 O3 Si1 -171.9(17) . . . . ?
Na1 Si2 O3 Si1 95.9(15) 3_565 . . . ?
Na4 Si2 O3 Si1 19.8(18) 3_565 . . . ?
Na4 Si2 O3 Si1 -84.0(15) 4_655 . . . ?
Eu3 Si2 O3 Si1 -99.5(15) . . . . ?
Eu1 Si2 O3 Si1 -179.9(14) 3_565 . . . ?
Eu2 Si2 O3 Si1 57.4(15) 3_565 . . . ?
O6 Si2 O3 Na4 -110.1(2) . . . . ?
O4 Si2 O3 Na4 17.7(3) . . . . ?
O5 Si2 O3 Na4 129.3(3) . . . . ?
Na1 Si2 O3 Na4 -92.25(19) 3_565 . . . ?
Na4 Si2 O3 Na4 -168.29(18) 3_565 . . . ?
Na4 Si2 O3 Na4 87.88(19) 4_655 . . . ?
Eu3 Si2 O3 Na4 72.4(3) . . . . ?
Eu1 Si2 O3 Na4 -8.0(3) 3_565 . . . ?
Eu2 Si2 O3 Na4 -130.76(16) 3_565 . . . ?
O6 Si2 O3 Na1 -17.9(3) . . . 3_565 ?
O4 Si2 O3 Na1 110.0(2) . . . 3_565 ?
O5 Si2 O3 Na1 -138.4(3) . . . 3_565 ?
Na4 Si2 O3 Na1 92.25(19) . . . 3_565 ?
Na4 Si2 O3 Na1 -76.0(3) 3_565 . . 3_565 ?
Na4 Si2 O3 Na1 -179.9(2) 4_655 . . 3_565 ?
Eu3 Si2 O3 Na1 164.62(11) . . . 3_565 ?
Eu1 Si2 O3 Na1 84.27(18) 3_565 . . 3_565 ?
Eu2 Si2 O3 Na1 -38.51(14) 3_565 . . 3_565 ?
O6 Si2 O3 Na4 162.0(2) . . . 4_655 ?
O4 Si2 O3 Na4 -70.1(2) . . . 4_655 ?
O5 Si2 O3 Na4 41.5(3) . . . 4_655 ?
Na4 Si2 O3 Na4 -87.88(19) . . . 4_655 ?
Na1 Si2 O3 Na4 179.9(2) 3_565 . . 4_655 ?
Na4 Si2 O3 Na4 103.8(3) 3_565 . . 4_655 ?
Eu3 Si2 O3 Na4 -15.5(3) . . . 4_655 ?
Eu1 Si2 O3 Na4 -95.86(14) 3_565 . . 4_655 ?
Eu2 Si2 O3 Na4 141.36(10) 3_565 . . 4_655 ?
O6 Na4 O3 Si1 -95.6(3) 2_765 . . . ?
O6 Na4 O3 Si1 81.2(3) 3_465 . . . ?
O4 Na4 O3 Si1 165.9(3) . . . . ?
O1 Na4 O3 Si1 165.6(2) 7_755 . . . ?
O2 Na4 O3 Si1 -14.0(2) . . . . ?
O5 Na4 O3 Si1 35.0(4) 3_465 . . . ?
O3 Na4 O3 Si1 -40.4(18) 4_645 . . . ?
Eu2 Na4 O3 Si1 126.9(2) . . . . ?
Si2 Na4 O3 Si1 177.7(5) . . . . ?
O6 Na4 O3 Si2 86.6(3) 2_765 . . . ?
O6 Na4 O3 Si2 -96.5(3) 3_465 . . . ?
O4 Na4 O3 Si2 -11.8(2) . . . . ?
O1 Na4 O3 Si2 -12.1(4) 7_755 . . . ?
O2 Na4 O3 Si2 168.3(3) . . . . ?
O5 Na4 O3 Si2 -142.8(3) 3_465 . . . ?
O3 Na4 O3 Si2 141.9(15) 4_645 . . . ?
Eu2 Na4 O3 Si2 -50.8(2) . . . . ?
Si1 Na4 O3 Si2 -177.7(5) . . . . ?
O6 Na4 O3 Na1 -8.09(16) 2_765 . . 3_565 ?
O6 Na4 O3 Na1 168.80(15) 3_465 . . 3_565 ?
O4 Na4 O3 Na1 -106.53(17) . . . 3_565 ?
O1 Na4 O3 Na1 -106.8(2) 7_755 . . 3_565 ?
O2 Na4 O3 Na1 73.59(18) . . . 3_565 ?
O5 Na4 O3 Na1 122.5(2) 3_465 . . 3_565 ?
O3 Na4 O3 Na1 47.2(16) 4_645 . . 3_565 ?
Eu2 Na4 O3 Na1 -145.55(11) . . . 3_565 ?
Si2 Na4 O3 Na1 -94.7(3) . . . 3_565 ?
Si1 Na4 O3 Na1 87.6(2) . . . 3_565 ?
O6 Na4 O3 Na4 173.76(19) 2_765 . . 4_655 ?
O6 Na4 O3 Na4 -9.35(12) 3_465 . . 4_655 ?
O4 Na4 O3 Na4 75.31(15) . . . 4_655 ?
O1 Na4 O3 Na4 75.0(2) 7_755 . . 4_655 ?
O2 Na4 O3 Na4 -104.6(2) . . . 4_655 ?
O5 Na4 O3 Na4 -55.6(2) 3_465 . . 4_655 ?
O3 Na4 O3 Na4 -131.0(17) 4_645 . . 4_655 ?
Eu2 Na4 O3 Na4 36.30(10) . . . 4_655 ?
Si2 Na4 O3 Na4 87.1(2) . . . 4_655 ?
Si1 Na4 O3 Na4 -90.6(3) . . . 4_655 ?
O6 Si2 O4 Eu1 5.3(5) . . . 3_565 ?
O5 Si2 O4 Eu1 129.2(3) . . . 3_565 ?
O3 Si2 O4 Eu1 -118.5(4) . . . 3_565 ?
Na4 Si2 O4 Eu1 -101.6(4) . . . 3_565 ?
Na1 Si2 O4 Eu1 -60.4(4) 3_565 . . 3_565 ?
Na4 Si2 O4 Eu1 65.6(4) 3_565 . . 3_565 ?
Na4 Si2 O4 Eu1 -176.1(4) 4_655 . . 3_565 ?
Eu3 Si2 O4 Eu1 109.6(4) . . . 3_565 ?
Eu2 Si2 O4 Eu1 5.1(5) 3_565 . . 3_565 ?
O6 Si2 O4 Eu2 179.3(3) . . . . ?
O5 Si2 O4 Eu2 -56.8(4) . . . . ?
O3 Si2 O4 Eu2 55.5(4) . . . . ?
Na4 Si2 O4 Eu2 72.4(3) . . . . ?
Na1 Si2 O4 Eu2 113.6(3) 3_565 . . . ?
Na4 Si2 O4 Eu2 -120.4(3) 3_565 . . . ?
Na4 Si2 O4 Eu2 -2.1(3) 4_655 . . . ?
Eu3 Si2 O4 Eu2 -76.4(3) . . . . ?
Eu1 Si2 O4 Eu2 174.0(7) 3_565 . . . ?
Eu2 Si2 O4 Eu2 179.12(14) 3_565 . . . ?
O6 Si2 O4 Na4 107.0(3) . . . . ?
O5 Si2 O4 Na4 -129.15(15) . . . . ?
O3 Si2 O4 Na4 -16.8(3) . . . . ?
Na1 Si2 O4 Na4 41.21(18) 3_565 . . . ?
Na4 Si2 O4 Na4 167.23(10) 3_565 . . . ?
Na4 Si2 O4 Na4 -74.46(10) 4_655 . . . ?
Eu3 Si2 O4 Na4 -148.8(2) . . . . ?
Eu1 Si2 O4 Na4 101.6(4) 3_565 . . . ?
Eu2 Si2 O4 Na4 106.8(2) 3_565 . . . ?
O6 Si2 O4 Eu3 -104.3(3) . . . . ?
O5 Si2 O4 Eu3 19.6(2) . . . . ?
O3 Si2 O4 Eu3 131.9(2) . . . . ?
Na4 Si2 O4 Eu3 148.8(2) . . . . ?
Na1 Si2 O4 Eu3 -170.03(6) 3_565 . . . ?
Na4 Si2 O4 Eu3 -44.01(18) 3_565 . . . ?
Na4 Si2 O4 Eu3 74.29(12) 4_655 . . . ?
Eu1 Si2 O4 Eu3 -109.6(4) 3_565 . . . ?
Eu2 Si2 O4 Eu3 -104.5(2) 3_565 . . . ?
O6 Eu2 O4 Si2 151.5(5) 8_575 . . . ?
O6 Eu2 O4 Si2 -37.7(4) 3_465 . . . ?
O2 Eu2 O4 Si2 53.9(4) 7_765 . . . ?
O1 Eu2 O4 Si2 -137.8(4) 7_755 . . . ?
O4 Eu2 O4 Si2 144.2(3) 6 . . . ?
Na4 Eu2 O4 Si2 -179.0(3) 6 . . . ?
Na4 Eu2 O4 Si2 -79.4(3) . . . . ?
Eu3 Eu2 O4 Si2 85.4(3) . . . . ?
Na1 Eu2 O4 Si2 -0.7(5) . . . . ?
Na4 Eu2 O4 Si2 2.2(3) 4_655 . . . ?
Na4 Eu2 O4 Si2 98.5(4) 7_765 . . . ?
O6 Eu2 O4 Eu1 -32.7(6) 8_575 . . 3_565 ?
O6 Eu2 O4 Eu1 138.08(16) 3_465 . . 3_565 ?
O2 Eu2 O4 Eu1 -130.27(13) 7_765 . . 3_565 ?
O1 Eu2 O4 Eu1 38.02(12) 7_755 . . 3_565 ?
O4 Eu2 O4 Eu1 -39.97(17) 6 . . 3_565 ?
Na4 Eu2 O4 Eu1 -3.17(15) 6 . . 3_565 ?
Na4 Eu2 O4 Eu1 96.45(14) . . . 3_565 ?
Eu3 Eu2 O4 Eu1 -98.82(13) . . . 3_565 ?
Na1 Eu2 O4 Eu1 175.16(8) . . . 3_565 ?
Na4 Eu2 O4 Eu1 178.01(15) 4_655 . . 3_565 ?
Na4 Eu2 O4 Eu1 -85.69(14) 7_765 . . 3_565 ?
O6 Eu2 O4 Na4 -129.1(6) 8_575 . . . ?
O6 Eu2 O4 Na4 41.62(15) 3_465 . . . ?
O2 Eu2 O4 Na4 133.27(11) 7_765 . . . ?
O1 Eu2 O4 Na4 -58.44(11) 7_755 . . . ?
O4 Eu2 O4 Na4 -136.42(8) 6 . . . ?
Na4 Eu2 O4 Na4 -99.62(12) 6 . . . ?
Eu3 Eu2 O4 Na4 164.73(13) . . . . ?
Na1 Eu2 O4 Na4 78.70(17) . . . . ?
Na4 Eu2 O4 Na4 81.55(7) 4_655 . . . ?
Na4 Eu2 O4 Na4 177.86(11) 7_765 . . . ?
O6 Eu2 O4 Eu3 66.1(6) 8_575 . . . ?
O6 Eu2 O4 Eu3 -123.10(14) 3_465 . . . ?
O2 Eu2 O4 Eu3 -31.46(10) 7_765 . . . ?
O1 Eu2 O4 Eu3 136.84(12) 7_755 . . . ?
O4 Eu2 O4 Eu3 58.85(11) 6 . . . ?
Na4 Eu2 O4 Eu3 95.65(9) 6 . . . ?
Na4 Eu2 O4 Eu3 -164.73(13) . . . . ?
Na1 Eu2 O4 Eu3 -86.02(15) . . . . ?
Na4 Eu2 O4 Eu3 -83.17(8) 4_655 . . . ?
Na4 Eu2 O4 Eu3 13.13(14) 7_765 . . . ?
O6 Na4 O4 Si2 -75.4(2) 2_765 . . . ?
O3 Na4 O4 Si2 12.1(2) . . . . ?
O6 Na4 O4 Si2 101.90(19) 3_465 . . . ?
O1 Na4 O4 Si2 -168.2(2) 7_755 . . . ?
O2 Na4 O4 Si2 12.2(3) . . . . ?
O5 Na4 O4 Si2 121.0(3) 3_465 . . . ?
O3 Na4 O4 Si2 -165.02(19) 4_645 . . . ?
Eu2 Na4 O4 Si2 138.1(2) . . . . ?
Si1 Na4 O4 Si2 19.02(18) . . . . ?
O6 Na4 O4 Eu1 61.37(19) 2_765 . . 3_565 ?
O3 Na4 O4 Eu1 148.8(2) . . . 3_565 ?
O6 Na4 O4 Eu1 -121.33(16) 3_465 . . 3_565 ?
O1 Na4 O4 Eu1 -31.41(16) 7_755 . . 3_565 ?
O2 Na4 O4 Eu1 148.94(17) . . . 3_565 ?
O5 Na4 O4 Eu1 -102.2(3) 3_465 . . 3_565 ?
O3 Na4 O4 Eu1 -28.3(2) 4_645 . . 3_565 ?
Eu2 Na4 O4 Eu1 -85.13(12) . . . 3_565 ?
Si2 Na4 O4 Eu1 136.8(3) . . . 3_565 ?
Si1 Na4 O4 Eu1 155.79(12) . . . 3_565 ?
O6 Na4 O4 Eu2 146.51(17) 2_765 . . . ?
O3 Na4 O4 Eu2 -126.04(18) . . . . ?
O6 Na4 O4 Eu2 -36.20(12) 3_465 . . . ?
O1 Na4 O4 Eu2 53.72(14) 7_755 . . . ?
O2 Na4 O4 Eu2 -125.92(17) . . . . ?
O5 Na4 O4 Eu2 -17.1(3) 3_465 . . . ?
O3 Na4 O4 Eu2 56.88(19) 4_645 . . . ?
Si2 Na4 O4 Eu2 -138.1(2) . . . . ?
Si1 Na4 O4 Eu2 -119.07(9) . . . . ?
O6 Na4 O4 Eu3 174.2(3) 2_765 . . . ?
O3 Na4 O4 Eu3 -98.4(3) . . . . ?
O6 Na4 O4 Eu3 -8.5(3) 3_465 . . . ?
O1 Na4 O4 Eu3 81.4(3) 7_755 . . . ?
O2 Na4 O4 Eu3 -98.3(3) . . . . ?
O5 Na4 O4 Eu3 10.6(5) 3_465 . . . ?
O3 Na4 O4 Eu3 84.5(3) 4_645 . . . ?
Eu2 Na4 O4 Eu3 27.6(2) . . . . ?
Si2 Na4 O4 Eu3 -110.4(4) . . . . ?
Si1 Na4 O4 Eu3 -91.4(3) . . . . ?
O2 Eu3 O4 Si2 76.02(19) 3_565 . . . ?
O2 Eu3 O4 Si2 -103.98(19) 7_765 . . . ?
O4 Eu3 O4 Si2 166.66(12) 6 . . . ?
O4 Eu3 O4 Si2 -13.34(12) 2_775 . . . ?
O4 Eu3 O4 Si2 -113(93) 5_775 . . . ?
O5 Eu3 O4 Si2 166.66(12) 5_775 . . . ?
O5 Eu3 O4 Si2 -13.34(12) . . . . ?
Eu2 Eu3 O4 Si2 -137.0(2) . . . . ?
Eu2 Eu3 O4 Si2 43.0(2) 5_775 . . . ?
Si2 Eu3 O4 Si2 160.32(17) 6 . . . ?
Si2 Eu3 O4 Si2 -19.68(17) 2_775 . . . ?
O2 Eu3 O4 Eu1 -62.55(14) 3_565 . . 3_565 ?
O2 Eu3 O4 Eu1 117.45(14) 7_765 . . 3_565 ?
O4 Eu3 O4 Eu1 28.09(17) 6 . . 3_565 ?
O4 Eu3 O4 Eu1 -151.91(17) 2_775 . . 3_565 ?
O4 Eu3 O4 Eu1 109(100) 5_775 . . 3_565 ?
O5 Eu3 O4 Eu1 28.09(17) 5_775 . . 3_565 ?
O5 Eu3 O4 Eu1 -151.91(17) . . . 3_565 ?
Eu2 Eu3 O4 Eu1 84.46(12) . . . 3_565 ?
Eu2 Eu3 O4 Eu1 -95.54(12) 5_775 . . 3_565 ?
Si2 Eu3 O4 Eu1 21.74(13) 6 . . 3_565 ?
Si2 Eu3 O4 Eu1 -158.26(13) 2_775 . . 3_565 ?
O2 Eu3 O4 Eu2 -147.02(10) 3_565 . . . ?
O2 Eu3 O4 Eu2 32.98(10) 7_765 . . . ?
O4 Eu3 O4 Eu2 -56.37(12) 6 . . . ?
O4 Eu3 O4 Eu2 123.63(12) 2_775 . . . ?
O4 Eu3 O4 Eu2 24(72) 5_775 . . . ?
O5 Eu3 O4 Eu2 -56.37(12) 5_775 . . . ?
O5 Eu3 O4 Eu2 123.63(12) . . . . ?
Eu2 Eu3 O4 Eu2 180.0 5_775 . . . ?
Si2 Eu3 O4 Eu2 -62.72(8) 6 . . . ?
Si2 Eu3 O4 Eu2 117.28(8) 2_775 . . . ?
O2 Eu3 O4 Na4 -174.7(3) 3_565 . . . ?
O2 Eu3 O4 Na4 5.3(3) 7_765 . . . ?
O4 Eu3 O4 Na4 -84.1(3) 6 . . . ?
O4 Eu3 O4 Na4 95.9(3) 2_775 . . . ?
O4 Eu3 O4 Na4 -3(100) 5_775 . . . ?
O5 Eu3 O4 Na4 -84.1(3) 5_775 . . . ?
O5 Eu3 O4 Na4 95.9(3) . . . . ?
Eu2 Eu3 O4 Na4 -27.7(2) . . . . ?
Eu2 Eu3 O4 Na4 152.3(2) 5_775 . . . ?
Si2 Eu3 O4 Na4 -90.4(3) 6 . . . ?
Si2 Eu3 O4 Na4 89.6(3) 2_775 . . . ?
O6 Si2 O5 Si2 -71.5(2) . . . 2_775 ?
O4 Si2 O5 Si2 160.73(18) . . . 2_775 ?
O3 Si2 O5 Si2 48.8(2) . . . 2_775 ?
Na4 Si2 O5 Si2 102.5(3) . . . 2_775 ?
Na1 Si2 O5 Si2 -6.07(9) 3_565 . . 2_775 ?
Na4 Si2 O5 Si2 -91.8(2) 3_565 . . 2_775 ?
Na4 Si2 O5 Si2 91.7(2) 4_655 . . 2_775 ?
Eu3 Si2 O5 Si2 180.000(6) . . . 2_775 ?
Eu1 Si2 O5 Si2 -175.89(6) 3_565 . . 2_775 ?
Eu2 Si2 O5 Si2 -50.61(5) 3_565 . . 2_775 ?
O6 Si2 O5 Eu3 108.5(2) . . . . ?
O4 Si2 O5 Eu3 -19.27(18) . . . . ?
O3 Si2 O5 Eu3 -131.2(2) . . . . ?
Na4 Si2 O5 Eu3 -77.5(3) . . . . ?
Na1 Si2 O5 Eu3 173.93(9) 3_565 . . . ?
Na4 Si2 O5 Eu3 88.22(19) 3_565 . . . ?
Na4 Si2 O5 Eu3 -88.3(2) 4_655 . . . ?
Eu1 Si2 O5 Eu3 4.11(6) 3_565 . . . ?
Eu2 Si2 O5 Eu3 129.39(5) 3_565 . . . ?
O6 Si2 O5 Na4 -163.2(2) . . . 4_655 ?
O4 Si2 O5 Na4 69.0(3) . . . 4_655 ?
O3 Si2 O5 Na4 -42.9(3) . . . 4_655 ?
Na4 Si2 O5 Na4 10.8(5) . . . 4_655 ?
Na1 Si2 O5 Na4 -97.76(18) 3_565 . . 4_655 ?
Na4 Si2 O5 Na4 176.5(4) 3_565 . . 4_655 ?
Eu3 Si2 O5 Na4 88.3(2) . . . 4_655 ?
Eu1 Si2 O5 Na4 92.42(19) 3_565 . . 4_655 ?
Eu2 Si2 O5 Na4 -142.30(17) 3_565 . . 4_655 ?
O6 Si2 O5 Na4 20.2(4) . . . 3_565 ?
O4 Si2 O5 Na4 -107.5(2) . . . 3_565 ?
O3 Si2 O5 Na4 140.6(2) . . . 3_565 ?
Na4 Si2 O5 Na4 -165.75(13) . . . 3_565 ?
Na1 Si2 O5 Na4 85.7(2) 3_565 . . 3_565 ?
Na4 Si2 O5 Na4 -176.5(4) 4_655 . . 3_565 ?
Eu3 Si2 O5 Na4 -88.22(19) . . . 3_565 ?
Eu1 Si2 O5 Na4 -84.1(2) 3_565 . . 3_565 ?
Eu2 Si2 O5 Na4 41.2(2) 3_565 . . 3_565 ?
O2 Eu3 O5 Si2 -78.03(15) 3_565 . . . ?
O2 Eu3 O5 Si2 101.97(15) 7_765 . . . ?
O4 Eu3 O5 Si2 13.13(12) 6 . . . ?
O4 Eu3 O5 Si2 -166.87(12) 2_775 . . . ?
O4 Eu3 O5 Si2 13.13(12) . . . . ?
O4 Eu3 O5 Si2 -166.87(12) 5_775 . . . ?
O5 Eu3 O5 Si2 87(100) 5_775 . . . ?
Eu2 Eu3 O5 Si2 53.04(5) . . . . ?
Eu2 Eu3 O5 Si2 -126.96(5) 5_775 . . . ?
Si2 Eu3 O5 Si2 0.000(2) 6 . . . ?
Si2 Eu3 O5 Si2 180.000(1) 2_775 . . . ?
O2 Eu3 O5 Si2 101.97(15) 3_565 . . 2_775 ?
O2 Eu3 O5 Si2 -78.03(15) 7_765 . . 2_775 ?
O4 Eu3 O5 Si2 -166.87(12) 6 . . 2_775 ?
O4 Eu3 O5 Si2 13.13(12) 2_775 . . 2_775 ?
O4 Eu3 O5 Si2 -166.87(12) . . . 2_775 ?
O4 Eu3 O5 Si2 13.13(12) 5_775 . . 2_775 ?
O5 Eu3 O5 Si2 -93(100) 5_775 . . 2_775 ?
Eu2 Eu3 O5 Si2 -126.96(5) . . . 2_775 ?
Eu2 Eu3 O5 Si2 53.04(5) 5_775 . . 2_775 ?
Si2 Eu3 O5 Si2 180.000(1) 6 . . 2_775 ?
O2 Eu3 O5 Na4 -168.47(15) 3_565 . . 4_655 ?
O2 Eu3 O5 Na4 11.53(15) 7_765 . . 4_655 ?
O4 Eu3 O5 Na4 -77.31(12) 6 . . 4_655 ?
O4 Eu3 O5 Na4 102.69(12) 2_775 . . 4_655 ?
O4 Eu3 O5 Na4 -77.31(12) . . . 4_655 ?
O4 Eu3 O5 Na4 102.69(12) 5_775 . . 4_655 ?
O5 Eu3 O5 Na4 -4(100) 5_775 . . 4_655 ?
Eu2 Eu3 O5 Na4 -37.40(6) . . . 4_655 ?
Eu2 Eu3 O5 Na4 142.60(6) 5_775 . . 4_655 ?
Si2 Eu3 O5 Na4 -90.44(7) 6 . . 4_655 ?
Si2 Eu3 O5 Na4 89.56(7) 2_775 . . 4_655 ?
O2 Eu3 O5 Na4 11.53(15) 3_565 . . 3_565 ?
O2 Eu3 O5 Na4 -168.47(15) 7_765 . . 3_565 ?
O4 Eu3 O5 Na4 102.69(12) 6 . . 3_565 ?
O4 Eu3 O5 Na4 -77.31(12) 2_775 . . 3_565 ?
O4 Eu3 O5 Na4 102.69(12) . . . 3_565 ?
O4 Eu3 O5 Na4 -77.31(12) 5_775 . . 3_565 ?
O5 Eu3 O5 Na4 176(100) 5_775 . . 3_565 ?
Eu2 Eu3 O5 Na4 142.60(6) . . . 3_565 ?
Eu2 Eu3 O5 Na4 -37.40(6) 5_775 . . 3_565 ?
Si2 Eu3 O5 Na4 89.56(7) 6 . . 3_565 ?
Si2 Eu3 O5 Na4 -90.44(7) 2_775 . . 3_565 ?
O4 Si2 O6 Na2 -179.7(4) . . . 3_565 ?
O5 Si2 O6 Na2 59.4(6) . . . 3_565 ?
O3 Si2 O6 Na2 -58.4(6) . . . 3_565 ?
Na4 Si2 O6 Na2 -115.5(4) . . . 3_565 ?
Na1 Si2 O6 Na2 -75.5(4) 3_565 . . 3_565 ?
Na4 Si2 O6 Na2 81.1(5) 3_565 . . 3_565 ?
Na4 Si2 O6 Na2 5.0(12) 4_655 . . 3_565 ?
Eu3 Si2 O6 Na2 119.6(4) . . . 3_565 ?
Eu1 Si2 O6 Na2 -177.3(5) 3_565 . . 3_565 ?
Eu2 Si2 O6 Na2 0.000(1) 3_565 . . 3_565 ?
O4 Si2 O6 Eu2 -179.7(4) . . . 3_565 ?
O5 Si2 O6 Eu2 59.4(6) . . . 3_565 ?
O3 Si2 O6 Eu2 -58.4(6) . . . 3_565 ?
Na4 Si2 O6 Eu2 -115.5(4) . . . 3_565 ?
Na1 Si2 O6 Eu2 -75.5(4) 3_565 . . 3_565 ?
Na4 Si2 O6 Eu2 81.1(5) 3_565 . . 3_565 ?
Na4 Si2 O6 Eu2 5.0(12) 4_655 . . 3_565 ?
Eu3 Si2 O6 Eu2 119.6(4) . . . 3_565 ?
Eu1 Si2 O6 Eu2 -177.3(5) 3_565 . . 3_565 ?
O4 Si2 O6 Na4 -7.8(5) . . . 2_765 ?
O5 Si2 O6 Na4 -128.7(5) . . . 2_765 ?
O3 Si2 O6 Na4 113.5(4) . . . 2_765 ?
Na4 Si2 O6 Na4 56.4(4) . . . 2_765 ?
Na1 Si2 O6 Na4 96.4(4) 3_565 . . 2_765 ?
Na4 Si2 O6 Na4 -107.1(4) 3_565 . . 2_765 ?
Na4 Si2 O6 Na4 176.9(4) 4_655 . . 2_765 ?
Eu3 Si2 O6 Na4 -68.5(4) . . . 2_765 ?
Eu1 Si2 O6 Na4 -5.4(4) 3_565 . . 2_765 ?
Eu2 Si2 O6 Na4 171.9(8) 3_565 . . 2_765 ?
O4 Si2 O6 Na4 99.3(2) . . . 3_565 ?
O5 Si2 O6 Na4 -21.7(4) . . . 3_565 ?
O3 Si2 O6 Na4 -139.4(2) . . . 3_565 ?
Na4 Si2 O6 Na4 163.46(8) . . . 3_565 ?
Na1 Si2 O6 Na4 -156.6(2) 3_565 . . 3_565 ?
Na4 Si2 O6 Na4 -76.1(7) 4_655 . . 3_565 ?
Eu3 Si2 O6 Na4 38.5(2) . . . 3_565 ?
Eu1 Si2 O6 Na4 101.62(13) 3_565 . . 3_565 ?
Eu2 Si2 O6 Na4 -81.1(5) 3_565 . . 3_565 ?
O4 Si2 O6 Na1 -104.2(2) . . . 3_565 ?
O5 Si2 O6 Na1 134.9(3) . . . 3_565 ?
O3 Si2 O6 Na1 17.1(2) . . . 3_565 ?
Na4 Si2 O6 Na1 -39.99(19) . . . 3_565 ?
Na4 Si2 O6 Na1 156.6(2) 3_565 . . 3_565 ?
Na4 Si2 O6 Na1 80.5(7) 4_655 . . 3_565 ?
Eu3 Si2 O6 Na1 -164.92(7) . . . 3_565 ?
Eu1 Si2 O6 Na1 -101.83(10) 3_565 . . 3_565 ?
Eu2 Si2 O6 Na1 75.5(4) 3_565 . . 3_565 ?

_diffrn_measured_fraction_theta_max 1.000
_diffrn_reflns_theta_full        25.02
_diffrn_measured_fraction_theta_full 1.000
_refine_diff_density_max         0.707
_refine_diff_density_min         -0.490
_refine_diff_density_rms         0.161
_database_code_depnum_ccdc_archive 'CCDC 1007245'
#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_101_04

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Eu F K2 O10 Si4'
_chemical_formula_weight         521.52

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Eu Eu -0.1578 3.6682 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Monoclinic
_symmetry_space_group_name_H-M   P21/m

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z'
'-x, -y, -z'
'x, -y-1/2, z'

_cell_length_a                   11.6796(8)
_cell_length_b                   8.5399(6)
_cell_length_c                   11.7874(8)
_cell_angle_alpha                90.00
_cell_angle_beta                 112.7200(10)
_cell_angle_gamma                90.00
_cell_volume                     1084.47(13)
_cell_formula_units_Z            4
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    3347
_cell_measurement_theta_min      6.264
_cell_measurement_theta_max      50.230

_exptl_crystal_description       rod
_exptl_crystal_colour            colorless
_exptl_crystal_size_max          0.16
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.05
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    3.194
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             984
_exptl_absorpt_coefficient_mu    7.051
_exptl_absorpt_correction_type   Multi-scan
_exptl_absorpt_correction_T_min  0.559
_exptl_absorpt_correction_T_max  0.703
_exptl_absorpt_process_details   ?

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  CCD
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            5638
_diffrn_reflns_av_R_equivalents  0.0191
_diffrn_reflns_av_sigmaI/netI    0.0220
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_theta_min         1.87
_diffrn_reflns_theta_max         25.14
_reflns_number_total             2074
_reflns_number_gt                1954
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    ?
_computing_publication_material  ?

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0321P)²+17.9298P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   none
_refine_ls_hydrogen_treatment    none
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         2074
_refine_ls_number_parameters     178
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0299
_refine_ls_R_factor_gt           0.0282
_refine_ls_wR_factor_ref         0.0804
_refine_ls_wR_factor_gt          0.0794
_refine_ls_goodness_of_fit_ref   1.065
_refine_ls_restrained_S_all      1.065
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Eu1 Eu 0.21060(3) -0.00501(4) 0.28857(3) 0.00695(12) Uani 1 1 d . . .
Si1 Si 0.28002(16) 0.0718(2) 0.03051(15) 0.0079(4) Uani 1 1 d . . .
Si2 Si 0.49029(15) -0.0701(2) 0.24288(16) 0.0071(4) Uani 1 1 d . . .
Si3 Si 0.74771(15) 0.0720(2) 0.37979(15) 0.0073(4) Uani 1 1 d . . .
Si4 Si 0.11103(15) 0.0644(2) -0.23554(15) 0.0068(4) Uani 1 1 d . . .
F1 F 0.1723(6) -0.2500 0.2157(6) 0.0201(13) Uani 1 2 d S . .
F2 F 0.2487(6) 0.2500 0.3434(6) 0.0212(13) Uani 1 2 d S . .
O1 O -0.0074(4) -0.0381(6) -0.2500(4) 0.0127(10) Uani 1 1 d . . .
O2 O 0.1798(4) 0.0541(6) 0.0891(4) 0.0140(10) Uani 1 1 d . . .
O3 O 0.4182(4) -0.0370(6) 0.3297(4) 0.0138(10) Uani 1 1 d . . .
O4 O 0.7507(5) 0.0462(6) 0.5123(4) 0.0163(10) Uani 1 1 d . . .
O5 O 0.3323(6) 0.2500 0.0375(7) 0.0161(15) Uani 1 2 d S . .
O6 O 0.2299(4) 0.0122(6) -0.1122(4) 0.0143(10) Uani 1 1 d . . .
O7 O 0.4045(4) -0.0369(6) 0.0979(4) 0.0109(9) Uani 1 1 d . . .
O8 O 0.6110(4) 0.0436(5) 0.2728(4) 0.0108(9) Uani 1 1 d . . .
O9 O 0.5395(6) -0.2500 0.2510(6) 0.0128(14) Uani 1 2 d S . .
O10 O 0.1508(4) 0.0394(6) -0.3526(4) 0.0127(10) Uani 1 1 d . . .
O11 O 0.0871(6) 0.2500 -0.2264(7) 0.0140(14) Uani 1 2 d S . .
O12 O 0.7859(6) 0.2500 0.3546(6) 0.0113(14) Uani 1 2 d S . .
K1 K 0.0573(2) 0.2500 0.4457(2) 0.0185(5) Uani 1 2 d S . .
K2 K 0.5885(2) 0.2500 0.0804(2) 0.0182(5) Uani 1 2 d S . .
K3 K 0.5089(2) 0.2500 0.4712(2) 0.0226(5) Uani 1 2 d S . .
K4 K 0.9668(2) 0.2500 0.0344(2) 0.0256(5) Uani 1 2 d S . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Eu1 F1 2.240(2) . ?
Eu1 O4 2.240(5) 3_656 ?
Eu1 F2 2.2664(18) . ?
Eu1 O1 2.267(4) 3 ?
Eu1 O2 2.293(5) . ?
Eu1 O3 2.298(4) . ?
Eu1 Si1 3.4993(17) . ?
Eu1 Si2 3.5536(17) . ?
Eu1 Si4 3.5980(17) 3 ?
Eu1 K1 3.7339(19) . ?
Eu1 K4 3.903(2) 1_455 ?
Eu1 K3 3.965(2) . ?
Si1 O2 1.580(5) . ?
Si1 O5 1.630(3) . ?
Si1 O6 1.634(5) . ?
Si1 O7 1.647(5) . ?
Si1 K2 3.629(2) 3_655 ?
Si1 K2 3.742(3) . ?
Si1 K4 3.840(2) 3_655 ?
Si2 O3 1.581(5) . ?
Si2 O9 1.630(3) . ?
Si2 O8 1.634(5) . ?
Si2 O7 1.637(5) . ?
Si2 K3 3.701(3) 3_656 ?
Si2 K2 3.762(2) . ?
Si2 K3 3.783(2) . ?
Si2 K2 3.875(3) 3_655 ?
Si3 O4 1.564(5) . ?
Si3 O8 1.626(5) . ?
Si3 O12 1.644(3) . ?
Si3 O10 1.646(5) 3_655 ?
Si3 K2 3.627(3) . ?
Si3 K1 3.655(2) 3_656 ?
Si3 K3 3.684(3) . ?
Si3 K1 3.717(3) 1_655 ?
Si4 O1 1.590(5) . ?
Si4 O11 1.620(2) . ?
Si4 O10 1.631(5) . ?
Si4 O6 1.637(5) . ?
Si4 Eu1 3.5980(17) 3 ?
Si4 K1 3.667(2) 3 ?
Si4 K1 3.899(3) 1_554 ?
Si4 K4 3.914(3) 3_655 ?
F1 Eu1 2.240(2) 4 ?
F1 K4 2.763(7) 3_655 ?
F2 Eu1 2.2664(17) 4_565 ?
F2 K3 2.823(7) . ?
F2 K1 2.921(7) . ?
O1 Eu1 2.267(4) 3 ?
O1 K1 2.810(5) 3 ?
O1 K4 3.005(5) 3_655 ?
O2 K4 2.857(5) 1_455 ?
O2 K4 3.142(5) 3_655 ?
O3 K3 2.828(5) 3_656 ?
O3 K3 2.923(5) . ?
O4 Eu1 2.240(5) 3_656 ?
O4 K3 3.191(5) . ?
O4 K1 3.288(5) 3_656 ?
O5 Si1 1.630(3) 4_565 ?
O5 K2 2.835(7) . ?
O6 K2 3.007(5) 3_655 ?
O7 K2 2.806(5) 3_655 ?
O7 K2 3.318(5) . ?
O8 K2 2.803(5) . ?
O9 Si2 1.630(3) 4 ?
O10 Si3 1.646(5) 3_655 ?
O10 K1 2.841(5) 1_554 ?
O10 K1 3.341(5) 3 ?
O11 Si4 1.620(2) 4_565 ?
O12 Si3 1.644(3) 4_565 ?
O12 K1 2.928(7) 1_655 ?
O12 K2 3.163(7) . ?
K1 O1 2.810(5) 3 ?
K1 O1 2.810(5) 2 ?
K1 O10 2.841(5) 4_566 ?
K1 O10 2.841(5) 1_556 ?
K1 O12 2.928(7) 1_455 ?
K1 O4 3.288(5) 2_656 ?
K1 O4 3.288(5) 3_656 ?
K1 O10 3.341(5) 3 ?
K1 O10 3.341(5) 2 ?
K1 Si3 3.655(2) 2_656 ?
K1 Si3 3.655(2) 3_656 ?
K2 O8 2.803(5) 4_565 ?
K2 O7 2.806(5) 3_655 ?
K2 O7 2.806(5) 2_655 ?
K2 O6 3.007(5) 2_655 ?
K2 O6 3.007(5) 3_655 ?
K2 O7 3.318(5) 4_565 ?
K2 Si3 3.627(3) 4_565 ?
K3 O3 2.828(5) 2_656 ?
K3 O3 2.828(5) 3_656 ?
K3 O3 2.923(5) 4_565 ?
K3 O4 3.191(5) 4_565 ?
K3 Si3 3.684(3) 4_565 ?
K3 Si2 3.701(3) 2_656 ?
K3 Si2 3.701(3) 3_656 ?
K4 F1 2.763(7) 3_655 ?
K4 O2 2.857(5) 4_665 ?
K4 O2 2.857(5) 1_655 ?
K4 O1 3.005(5) 2_655 ?
K4 O1 3.005(5) 3_655 ?
K4 O2 3.142(5) 3_655 ?
K4 O2 3.142(5) 2_655 ?
K4 Si1 3.840(2) 3_655 ?
K4 Si1 3.840(2) 2_655 ?
K4 Eu1 3.903(2) 4_665 ?
K4 Eu1 3.903(2) 1_655 ?
K4 Si4 3.914(3) 2_655 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F1 Eu1 O4 100.6(2) . 3_656 ?
F1 Eu1 F2 174.2(2) . . ?
O4 Eu1 F2 85.1(2) 3_656 . ?
F1 Eu1 O1 92.1(2) . 3 ?
O4 Eu1 O1 90.42(17) 3_656 3 ?
F2 Eu1 O1 88.64(19) . 3 ?
F1 Eu1 O2 83.31(19) . . ?
O4 Eu1 O2 175.67(18) 3_656 . ?
F2 Eu1 O2 91.0(2) . . ?
O1 Eu1 O2 91.21(16) 3 . ?
F1 Eu1 O3 90.5(2) . . ?
O4 Eu1 O3 89.49(17) 3_656 . ?
F2 Eu1 O3 88.8(2) . . ?
O1 Eu1 O3 177.44(17) 3 . ?
O2 Eu1 O3 88.70(16) . . ?
F1 Eu1 Si1 85.46(16) . . ?
O4 Eu1 Si1 156.87(13) 3_656 . ?
F2 Eu1 Si1 88.97(16) . . ?
O1 Eu1 Si1 111.80(12) 3 . ?
O2 Eu1 Si1 20.74(11) . . ?
O3 Eu1 Si1 68.02(12) . . ?
F1 Eu1 Si2 81.67(16) . . ?
O4 Eu1 Si2 108.01(13) 3_656 . ?
F2 Eu1 Si2 95.91(16) . . ?
O1 Eu1 Si2 161.31(12) 3 . ?
O2 Eu1 Si2 70.64(12) . . ?
O3 Eu1 Si2 19.37(12) . . ?
Si1 Eu1 Si2 50.39(4) . . ?
F1 Eu1 Si4 76.18(16) . 3 ?
O4 Eu1 Si4 86.23(13) 3_656 3 ?
F2 Eu1 Si4 105.17(16) . 3 ?
O1 Eu1 Si4 17.50(12) 3 3 ?
O2 Eu1 Si4 96.49(12) . 3 ?
O3 Eu1 Si4 164.94(13) . 3 ?
Si1 Eu1 Si4 116.89(4) . 3 ?
Si2 Eu1 Si4 155.61(4) . 3 ?
F1 Eu1 K1 132.21(16) . . ?
O4 Eu1 K1 60.86(13) 3_656 . ?
F2 Eu1 K1 51.46(16) . . ?
O1 Eu1 K1 48.66(12) 3 . ?
O2 Eu1 K1 117.70(12) . . ?
O3 Eu1 K1 129.33(13) . . ?
Si1 Eu1 K1 129.68(4) . . ?
Si2 Eu1 K1 144.23(4) . . ?
Si4 Eu1 K1 59.99(4) 3 . ?
F1 Eu1 K4 104.38(15) . 1_455 ?
O4 Eu1 K4 133.15(13) 3_656 1_455 ?
F2 Eu1 K4 71.79(15) . 1_455 ?
O1 Eu1 K4 50.12(13) 3 1_455 ?
O2 Eu1 K4 46.46(12) . 1_455 ?
O3 Eu1 K4 128.73(13) . 1_455 ?
Si1 Eu1 K4 64.76(5) . 1_455 ?
Si2 Eu1 K4 114.31(5) . 1_455 ?
Si4 Eu1 K4 62.75(4) 3 1_455 ?
K1 Eu1 K4 73.02(5) . 1_455 ?
F1 Eu1 K3 136.44(16) . . ?
O4 Eu1 K3 74.82(13) 3_656 . ?
F2 Eu1 K3 44.18(15) . . ?
O1 Eu1 K3 130.69(12) 3 . ?
O2 Eu1 K3 101.11(12) . . ?
O3 Eu1 K3 46.88(13) . . ?
Si1 Eu1 K3 85.35(5) . . ?
Si2 Eu1 K3 60.11(4) . . ?
Si4 Eu1 K3 144.22(4) 3 . ?
K1 Eu1 K3 84.24(4) . . ?
K4 Eu1 K3 109.74(3) 1_455 . ?
O2 Si1 O5 113.2(3) . . ?
O2 Si1 O6 112.9(3) . . ?
O5 Si1 O6 108.7(3) . . ?
O2 Si1 O7 113.6(3) . . ?
O5 Si1 O7 105.0(3) . . ?
O6 Si1 O7 102.7(2) . . ?
O2 Si1 Eu1 30.93(17) . . ?
O5 Si1 Eu1 109.8(3) . . ?
O6 Si1 Eu1 136.49(19) . . ?
O7 Si1 Eu1 86.13(16) . . ?
O2 Si1 K2 125.0(2) . 3_655 ?
O5 Si1 K2 121.5(2) . 3_655 ?
O6 Si1 K2 55.01(17) . 3_655 ?
O7 Si1 K2 47.93(17) . 3_655 ?
Eu1 Si1 K2 116.33(6) . 3_655 ?
O2 Si1 K2 143.2(2) . . ?
O5 Si1 K2 45.0(2) . . ?
O6 Si1 K2 103.23(18) . . ?
O7 Si1 K2 62.40(17) . . ?
Eu1 Si1 K2 118.15(6) . . ?
K2 Si1 K2 81.31(4) 3_655 . ?
O2 Si1 K4 52.60(19) . 3_655 ?
O5 Si1 K4 156.3(2) . 3_655 ?
O6 Si1 K4 68.22(18) . 3_655 ?
O7 Si1 K4 98.50(18) . 3_655 ?
Eu1 Si1 K4 68.35(5) . 3_655 ?
K2 Si1 K4 77.05(5) 3_655 3_655 ?
K2 Si1 K4 157.74(6) . 3_655 ?
O3 Si2 O9 113.2(3) . . ?
O3 Si2 O8 112.6(3) . . ?
O9 Si2 O8 107.0(3) . . ?
O3 Si2 O7 112.3(2) . . ?
O9 Si2 O7 106.5(3) . . ?
O8 Si2 O7 104.6(2) . . ?
O3 Si2 Eu1 28.82(17) . . ?
O9 Si2 Eu1 117.5(2) . . ?
O8 Si2 Eu1 129.88(18) . . ?
O7 Si2 Eu1 84.44(16) . . ?
O3 Si2 K3 45.54(18) . 3_656 ?
O9 Si2 K3 71.2(2) . 3_656 ?
O8 Si2 K3 110.60(18) . 3_656 ?
O7 Si2 K3 143.84(18) . 3_656 ?
Eu1 Si2 K3 66.79(5) . 3_656 ?
O3 Si2 K2 122.9(2) . . ?
O9 Si2 K2 123.0(2) . . ?
O8 Si2 K2 43.18(17) . . ?
O7 Si2 K2 61.77(18) . . ?
Eu1 Si2 K2 116.25(5) . . ?
K3 Si2 K2 150.61(6) 3_656 . ?
O3 Si2 K3 46.31(19) . . ?
O9 Si2 K3 135.8(3) . . ?
O8 Si2 K3 67.00(17) . . ?
O7 Si2 K3 117.45(18) . . ?
Eu1 Si2 K3 65.35(5) . . ?
K3 Si2 K3 70.91(3) 3_656 . ?
K2 Si2 K3 83.80(5) . . ?
O3 Si2 K2 136.35(19) . 3_655 ?
O9 Si2 K2 68.2(2) . 3_655 ?
O8 Si2 K2 107.76(17) . 3_655 ?
O7 Si2 K2 39.24(16) . 3_655 ?
Eu1 Si2 K2 109.15(5) . 3_655 ?
K3 Si2 K2 130.32(5) 3_656 3_655 ?
K2 Si2 K2 77.92(4) . 3_655 ?
K3 Si2 K2 155.86(6) . 3_655 ?
O4 Si3 O8 113.0(3) . . ?
O4 Si3 O12 114.1(3) . . ?
O8 Si3 O12 104.6(3) . . ?
O4 Si3 O10 111.9(3) . 3_655 ?
O8 Si3 O10 109.2(2) . 3_655 ?
O12 Si3 O10 103.5(3) . 3_655 ?
O4 Si3 K2 146.7(2) . . ?
O8 Si3 K2 47.68(17) . . ?
O12 Si3 K2 60.6(2) . . ?
O10 Si3 K2 100.96(17) 3_655 . ?
O4 Si3 K1 64.11(19) . 3_656 ?
O8 Si3 K1 122.43(19) . 3_656 ?
O12 Si3 K1 130.1(2) . 3_656 ?
O10 Si3 K1 48.35(17) 3_655 3_656 ?
K2 Si3 K1 146.80(6) . 3_656 ?
O4 Si3 K3 59.58(19) . . ?
O8 Si3 K3 70.17(17) . . ?
O12 Si3 K3 87.7(2) . . ?
O10 Si3 K3 168.38(19) 3_655 . ?
K2 Si3 K3 87.13(6) . . ?
K1 Si3 K3 121.56(6) 3_656 . ?
O4 Si3 K1 101.8(2) . 1_655 ?
O8 Si3 K1 143.87(18) . 1_655 ?
O12 Si3 K1 49.4(2) . 1_655 ?
O10 Si3 K1 63.97(18) 3_655 1_655 ?
K2 Si3 K1 97.11(6) . 1_655 ?
K1 Si3 K1 81.12(4) 3_656 1_655 ?
K3 Si3 K1 123.72(6) . 1_655 ?
O1 Si4 O11 112.3(3) . . ?
O1 Si4 O10 111.0(3) . . ?
O11 Si4 O10 107.3(3) . . ?
O1 Si4 O6 110.5(3) . . ?
O11 Si4 O6 108.4(3) . . ?
O10 Si4 O6 107.2(2) . . ?
O1 Si4 Eu1 25.40(18) . 3 ?
O11 Si4 Eu1 87.4(2) . 3 ?
O10 Si4 Eu1 116.99(18) . 3 ?
O6 Si4 Eu1 125.89(18) . 3 ?
O1 Si4 K1 46.15(18) . 3 ?
O11 Si4 K1 134.4(3) . 3 ?
O10 Si4 K1 65.56(18) . 3 ?
O6 Si4 K1 116.74(19) . 3 ?
Eu1 Si4 K1 61.84(4) 3 3 ?
O1 Si4 K1 108.11(19) . 1_554 ?
O11 Si4 K1 72.4(3) . 1_554 ?
O10 Si4 K1 39.66(17) . 1_554 ?
O6 Si4 K1 137.06(19) . 1_554 ?
Eu1 Si4 K1 96.96(5) 3 1_554 ?
K1 Si4 K1 78.57(4) 3 1_554 ?
O1 Si4 K4 44.87(18) . 3_655 ?
O11 Si4 K4 123.0(3) . 3_655 ?
O10 Si4 K4 129.16(19) . 3_655 ?
O6 Si4 K4 65.87(18) . 3_655 ?
Eu1 Si4 K4 62.44(4) 3 3_655 ?
K1 Si4 K4 73.60(5) 3 3_655 ?
K1 Si4 K4 150.92(6) 1_554 3_655 ?
Eu1 F1 Eu1 138.1(3) . 4 ?
Eu1 F1 K4 110.93(14) . 3_655 ?
Eu1 F1 K4 110.93(14) 4 3_655 ?
Eu1 F2 Eu1 147.9(3) . 4_565 ?
Eu1 F2 K3 101.80(15) . . ?
Eu1 F2 K3 101.80(15) 4_565 . ?
Eu1 F2 K1 91.18(16) . . ?
Eu1 F2 K1 91.18(16) 4_565 . ?
K3 F2 K1 128.1(2) . . ?
Si4 O1 Eu1 137.1(3) . 3 ?
Si4 O1 K1 109.8(2) . 3 ?
Eu1 O1 K1 94.07(16) 3 3 ?
Si4 O1 K4 113.2(2) . 3_655 ?
Eu1 O1 K4 94.49(16) 3 3_655 ?
K1 O1 K4 102.78(15) 3 3_655 ?
Si1 O2 Eu1 128.3(3) . . ?
Si1 O2 K4 125.0(2) . 1_455 ?
Eu1 O2 K4 97.96(16) . 1_455 ?
Si1 O2 K4 103.9(2) . 3_655 ?
Eu1 O2 K4 97.76(16) . 3_655 ?
K4 O2 K4 96.22(13) 1_455 3_655 ?
Si2 O3 Eu1 131.8(3) . . ?
Si2 O3 K3 110.9(2) . 3_656 ?
Eu1 O3 K3 101.89(17) . 3_656 ?
Si2 O3 K3 110.7(2) . . ?
Eu1 O3 K3 98.11(17) . . ?
K3 O3 K3 98.00(14) 3_656 . ?
Si3 O4 Eu1 170.4(3) . 3_656 ?
Si3 O4 K3 95.4(2) . . ?
Eu1 O4 K3 93.05(15) 3_656 . ?
Si3 O4 K1 90.6(2) . 3_656 ?
Eu1 O4 K1 82.63(15) 3_656 3_656 ?
K3 O4 K1 162.63(18) . 3_656 ?
Si1 O5 Si1 138.0(5) . 4_565 ?
Si1 O5 K2 111.0(2) . . ?
Si1 O5 K2 111.0(2) 4_565 . ?
Si1 O6 Si4 132.3(3) . . ?
Si1 O6 K2 98.5(2) . 3_655 ?
Si4 O6 K2 129.0(2) . 3_655 ?
Si2 O7 Si1 132.2(3) . . ?
Si2 O7 K2 119.1(2) . 3_655 ?
Si1 O7 K2 106.2(2) . 3_655 ?
Si2 O7 K2 92.5(2) . . ?
Si1 O7 K2 91.5(2) . . ?
K2 O7 K2 103.01(13) 3_655 . ?
Si3 O8 Si2 139.7(3) . . ?
Si3 O8 K2 106.9(2) . . ?
Si2 O8 K2 113.3(2) . . ?
Si2 O9 Si2 140.9(4) 4 . ?
Si4 O10 Si3 134.6(3) . 3_655 ?
Si4 O10 K1 118.8(2) . 1_554 ?
Si3 O10 K1 106.0(2) 3_655 1_554 ?
Si4 O10 K1 88.1(2) . 3 ?
Si3 O10 K1 89.8(2) 3_655 3 ?
K1 O10 K1 101.41(13) 1_554 3 ?
Si4 O11 Si4 156.1(5) 4_565 . ?
Si3 O12 Si3 135.3(4) . 4_565 ?
Si3 O12 K1 105.3(2) . 1_655 ?
Si3 O12 K1 105.3(2) 4_565 1_655 ?
Si3 O12 K2 92.5(2) . . ?
Si3 O12 K2 92.5(2) 4_565 . ?
K1 O12 K2 129.3(2) 1_655 . ?
O1 K1 O1 80.2(2) 3 2 ?
O1 K1 O10 170.15(16) 3 4_566 ?
O1 K1 O10 99.79(14) 2 4_566 ?
O1 K1 O10 99.79(14) 3 1_556 ?
O1 K1 O10 170.15(16) 2 1_556 ?
O10 K1 O10 78.5(2) 4_566 1_556 ?
O1 K1 F2 67.06(13) 3 . ?
O1 K1 F2 67.06(13) 2 . ?
O10 K1 F2 103.74(14) 4_566 . ?
O10 K1 F2 103.74(14) 1_556 . ?
O1 K1 O12 81.20(14) 3 1_455 ?
O1 K1 O12 81.20(14) 2 1_455 ?
O10 K1 O12 108.58(15) 4_566 1_455 ?
O10 K1 O12 108.58(15) 1_556 1_455 ?
F2 K1 O12 137.8(2) . 1_455 ?
O1 K1 O4 122.14(14) 3 2_656 ?
O1 K1 O4 62.69(13) 2 2_656 ?
O10 K1 O4 50.80(12) 4_566 2_656 ?
O10 K1 O4 109.98(15) 1_556 2_656 ?
F2 K1 O4 58.41(10) . 2_656 ?
O12 K1 O4 129.33(10) 1_455 2_656 ?
O1 K1 O4 62.69(13) 3 3_656 ?
O1 K1 O4 122.14(14) 2 3_656 ?
O10 K1 O4 109.98(15) 4_566 3_656 ?
O10 K1 O4 50.80(12) 1_556 3_656 ?
F2 K1 O4 58.41(10) . 3_656 ?
O12 K1 O4 129.33(10) 1_455 3_656 ?
O4 K1 O4 100.57(19) 2_656 3_656 ?
O1 K1 O10 50.21(12) 3 3 ?
O1 K1 O10 108.24(14) 2 3 ?
O10 K1 O10 137.63(9) 4_566 3 ?
O10 K1 O10 78.59(14) 1_556 3 ?
F2 K1 O10 116.10(11) . 3 ?
O12 K1 O10 48.11(8) 1_455 3 ?
O4 K1 O10 170.34(13) 2_656 3 ?
O4 K1 O10 81.22(12) 3_656 3 ?
O1 K1 O10 108.24(14) 3 2 ?
O1 K1 O10 50.21(12) 2 2 ?
O10 K1 O10 78.59(13) 4_566 2 ?
O10 K1 O10 137.63(9) 1_556 2 ?
F2 K1 O10 116.10(11) . 2 ?
O12 K1 O10 48.11(8) 1_455 2 ?
O4 K1 O10 81.22(12) 2_656 2 ?
O4 K1 O10 170.34(13) 3_656 2 ?
O10 K1 O10 95.45(17) 3 2 ?
O1 K1 Si3 146.40(12) 3 2_656 ?
O1 K1 Si3 82.18(10) 2 2_656 ?
O10 K1 Si3 25.64(9) 4_566 2_656 ?
O10 K1 Si3 92.91(12) 1_556 2_656 ?
F2 K1 Si3 79.77(9) . 2_656 ?
O12 K1 Si3 123.88(7) 1_455 2_656 ?
O4 K1 Si3 25.34(8) 2_656 2_656 ?
O4 K1 Si3 104.69(11) 3_656 2_656 ?
O10 K1 Si3 163.26(11) 3 2_656 ?
O10 K1 Si3 81.04(8) 2 2_656 ?
O1 K1 Si3 82.18(10) 3 3_656 ?
O1 K1 Si3 146.40(12) 2 3_656 ?
O10 K1 Si3 92.91(12) 4_566 3_656 ?
O10 K1 Si3 25.64(9) 1_556 3_656 ?
F2 K1 Si3 79.77(9) . 3_656 ?
O12 K1 Si3 123.88(7) 1_455 3_656 ?
O4 K1 Si3 104.69(11) 2_656 3_656 ?
O4 K1 Si3 25.34(8) 3_656 3_656 ?
O10 K1 Si3 81.04(8) 3 3_656 ?
O10 K1 Si3 163.26(11) 2 3_656 ?
Si3 K1 Si3 97.58(8) 2_656 3_656 ?
O8 K2 O8 77.9(2) 4_565 . ?
O8 K2 O7 173.36(16) 4_565 3_655 ?
O8 K2 O7 100.23(13) . 3_655 ?
O8 K2 O7 100.23(13) 4_565 2_655 ?
O8 K2 O7 173.36(16) . 2_655 ?
O7 K2 O7 80.9(2) 3_655 2_655 ?
O8 K2 O5 84.67(15) 4_565 . ?
O8 K2 O5 84.67(15) . . ?
O7 K2 O5 101.57(15) 3_655 . ?
O7 K2 O5 101.57(15) 2_655 . ?
O8 K2 O6 65.78(13) 4_565 2_655 ?
O8 K2 O6 121.75(15) . 2_655 ?
O7 K2 O6 110.67(15) 3_655 2_655 ?
O7 K2 O6 52.19(13) 2_655 2_655 ?
O5 K2 O6 131.87(10) . 2_655 ?
O8 K2 O6 121.75(15) 4_565 3_655 ?
O8 K2 O6 65.78(13) . 3_655 ?
O7 K2 O6 52.19(13) 3_655 3_655 ?
O7 K2 O6 110.67(15) 2_655 3_655 ?
O5 K2 O6 131.87(10) . 3_655 ?
O6 K2 O6 96.26(19) 2_655 3_655 ?
O8 K2 O12 50.95(12) 4_565 . ?
O8 K2 O12 50.95(12) . . ?
O7 K2 O12 123.01(13) 3_655 . ?
O7 K2 O12 123.01(13) 2_655 . ?
O5 K2 O12 119.0(2) . . ?
O6 K2 O12 70.83(12) 2_655 . ?
O6 K2 O12 70.83(12) 3_655 . ?
O8 K2 O7 105.93(13) 4_565 . ?
O8 K2 O7 49.14(12) . . ?
O7 K2 O7 76.99(13) 3_655 . ?
O7 K2 O7 137.13(9) 2_655 . ?
O5 K2 O7 49.22(9) . . ?
O6 K2 O7 170.06(14) 2_655 . ?
O6 K2 O7 83.40(12) 3_655 . ?
O12 K2 O7 99.81(12) . . ?
O8 K2 O7 49.14(12) 4_565 4_565 ?
O8 K2 O7 105.93(13) . 4_565 ?
O7 K2 O7 137.13(9) 3_655 4_565 ?
O7 K2 O7 76.99(13) 2_655 4_565 ?
O5 K2 O7 49.22(9) . 4_565 ?
O6 K2 O7 83.40(12) 2_655 4_565 ?
O6 K2 O7 170.06(14) 3_655 4_565 ?
O12 K2 O7 99.81(12) . 4_565 ?
O7 K2 O7 95.21(16) . 4_565 ?
O8 K2 Si3 25.40(9) 4_565 4_565 ?
O8 K2 Si3 67.90(11) . 4_565 ?
O7 K2 Si3 148.06(12) 3_655 4_565 ?
O7 K2 Si3 107.74(10) 2_655 4_565 ?
O5 K2 Si3 106.43(14) . 4_565 ?
O6 K2 Si3 59.64(10) 2_655 4_565 ?
O6 K2 Si3 96.82(11) 3_655 4_565 ?
O12 K2 Si3 26.92(5) . 4_565 ?
O7 K2 Si3 110.48(10) . 4_565 ?
O7 K2 Si3 74.39(9) 4_565 4_565 ?
O8 K2 Si3 67.90(11) 4_565 . ?
O8 K2 Si3 25.40(9) . . ?
O7 K2 Si3 107.74(10) 3_655 . ?
O7 K2 Si3 148.06(12) 2_655 . ?
O5 K2 Si3 106.43(14) . . ?
O6 K2 Si3 96.82(11) 2_655 . ?
O6 K2 Si3 59.64(10) 3_655 . ?
O12 K2 Si3 26.92(5) . . ?
O7 K2 Si3 74.39(9) . . ?
O7 K2 Si3 110.48(10) 4_565 . ?
Si3 K2 Si3 49.56(6) 4_565 . ?
F2 K3 O3 111.06(15) . 2_656 ?
F2 K3 O3 111.06(15) . 3_656 ?
O3 K3 O3 80.1(2) 2_656 3_656 ?
F2 K3 O3 67.50(11) . . ?
O3 K3 O3 159.92(14) 2_656 . ?
O3 K3 O3 82.00(14) 3_656 . ?
F2 K3 O3 67.50(11) . 4_565 ?
O3 K3 O3 82.00(14) 2_656 4_565 ?
O3 K3 O3 159.92(14) 3_656 4_565 ?
O3 K3 O3 113.9(2) . 4_565 ?
F2 K3 O4 142.03(12) . 4_565 ?
O3 K3 O4 63.79(13) 2_656 4_565 ?
O3 K3 O4 105.06(15) 3_656 4_565 ?
O3 K3 O4 130.42(14) . 4_565 ?
O3 K3 O4 74.57(13) 4_565 4_565 ?
F2 K3 O4 142.03(12) . . ?
O3 K3 O4 105.06(15) 2_656 . ?
O3 K3 O4 63.79(13) 3_656 . ?
O3 K3 O4 74.57(13) . . ?
O3 K3 O4 130.42(15) 4_565 . ?
O4 K3 O4 66.11(19) 4_565 . ?
F2 K3 Si3 128.66(13) . 4_565 ?
O3 K3 Si3 87.61(10) 2_656 4_565 ?
O3 K3 Si3 119.29(12) 3_656 4_565 ?
O3 K3 Si3 109.12(11) . 4_565 ?
O3 K3 Si3 68.63(10) 4_565 4_565 ?
O4 K3 Si3 25.01(9) 4_565 4_565 ?
O4 K3 Si3 62.87(10) . 4_565 ?
F2 K3 Si3 128.66(13) . . ?
O3 K3 Si3 119.29(12) 2_656 . ?
O3 K3 Si3 87.61(10) 3_656 . ?
O3 K3 Si3 68.63(10) . . ?
O3 K3 Si3 109.12(11) 4_565 . ?
O4 K3 Si3 62.87(10) 4_565 . ?
O4 K3 Si3 25.01(9) . . ?
Si3 K3 Si3 48.75(6) 4_565 . ?
F2 K3 Si2 96.27(14) . 2_656 ?
O3 K3 Si2 23.52(10) 2_656 2_656 ?
O3 K3 Si2 67.48(11) 3_656 2_656 ?
O3 K3 Si2 137.77(12) . 2_656 ?
O3 K3 Si2 92.55(10) 4_565 2_656 ?
O4 K3 Si2 86.82(9) 4_565 2_656 ?
O4 K3 Si2 113.42(11) . 2_656 ?
Si3 K3 Si2 111.05(5) 4_565 2_656 ?
Si3 K3 Si2 134.57(8) . 2_656 ?
F2 K3 Si2 96.27(14) . 3_656 ?
O3 K3 Si2 67.48(11) 2_656 3_656 ?
O3 K3 Si2 23.52(10) 3_656 3_656 ?
O3 K3 Si2 92.55(10) . 3_656 ?
O3 K3 Si2 137.77(12) 4_565 3_656 ?
O4 K3 Si2 113.42(11) 4_565 3_656 ?
O4 K3 Si2 86.82(9) . 3_656 ?
Si3 K3 Si2 134.57(8) 4_565 3_656 ?
Si3 K3 Si2 111.05(5) . 3_656 ?
Si2 K3 Si2 49.05(6) 2_656 3_656 ?
F2 K3 Si2 82.31(10) . . ?
O3 K3 Si2 166.26(13) 2_656 . ?
O3 K3 Si2 92.40(10) 3_656 . ?
O3 K3 Si2 23.02(9) . . ?
O3 K3 Si2 106.94(12) 4_565 . ?
O4 K3 Si2 107.86(11) 4_565 . ?
O4 K3 Si2 61.21(10) . . ?
Si3 K3 Si2 86.12(6) 4_565 . ?
Si3 K3 Si2 48.38(4) . . ?
Si2 K3 Si2 157.99(6) 2_656 . ?
Si2 K3 Si2 109.09(3) 3_656 . ?
F1 K4 O2 110.04(16) 3_655 4_665 ?
F1 K4 O2 110.04(16) 3_655 1_655 ?
O2 K4 O2 71.7(2) 4_665 1_655 ?
F1 K4 O1 137.58(12) 3_655 2_655 ?
O2 K4 O1 67.49(13) 4_665 2_655 ?
O2 K4 O1 108.82(15) 1_655 2_655 ?
F1 K4 O1 137.58(12) 3_655 3_655 ?
O2 K4 O1 108.82(15) 4_665 3_655 ?
O2 K4 O1 67.49(13) 1_655 3_655 ?
O1 K4 O1 74.08(19) 2_655 3_655 ?
F1 K4 O2 60.96(10) 3_655 3_655 ?
O2 K4 O2 149.29(12) 4_665 3_655 ?
O2 K4 O2 83.79(13) 1_655 3_655 ?
O1 K4 O2 140.33(15) 2_655 3_655 ?
O1 K4 O2 76.93(12) 3_655 3_655 ?
F1 K4 O2 60.96(10) 3_655 2_655 ?
O2 K4 O2 83.78(13) 4_665 2_655 ?
O2 K4 O2 149.29(12) 1_655 2_655 ?
O1 K4 O2 76.93(12) 2_655 2_655 ?
O1 K4 O2 140.33(15) 3_655 2_655 ?
O2 K4 O2 111.49(18) 3_655 2_655 ?
F1 K4 Si1 72.57(10) 3_655 3_655 ?
O2 K4 Si1 170.15(11) 4_665 3_655 ?
O2 K4 Si1 98.46(10) 1_655 3_655 ?
O1 K4 Si1 117.44(12) 2_655 3_655 ?
O1 K4 Si1 66.34(9) 3_655 3_655 ?
O2 K4 Si1 23.54(9) 3_655 3_655 ?
O2 K4 Si1 105.44(11) 2_655 3_655 ?
F1 K4 Si1 72.57(10) 3_655 2_655 ?
O2 K4 Si1 98.46(10) 4_665 2_655 ?
O2 K4 Si1 170.15(11) 1_655 2_655 ?
O1 K4 Si1 66.34(9) 2_655 2_655 ?
O1 K4 Si1 117.44(12) 3_655 2_655 ?
O2 K4 Si1 105.44(11) 3_655 2_655 ?
O2 K4 Si1 23.54(9) 2_655 2_655 ?
Si1 K4 Si1 91.39(7) 3_655 2_655 ?
F1 K4 Eu1 140.63(8) 3_655 4_665 ?
O2 K4 Eu1 35.58(9) 4_665 4_665 ?
O2 K4 Eu1 80.80(11) 1_655 4_665 ?
O1 K4 Eu1 35.38(9) 2_655 4_665 ?
O1 K4 Eu1 81.77(10) 3_655 4_665 ?
O2 K4 Eu1 157.28(10) 3_655 4_665 ?
O2 K4 Eu1 90.00(9) 2_655 4_665 ?
Si1 K4 Eu1 145.21(8) 3_655 4_665 ?
Si1 K4 Eu1 91.30(3) 2_655 4_665 ?
F1 K4 Eu1 140.63(8) 3_655 1_655 ?
O2 K4 Eu1 80.80(11) 4_665 1_655 ?
O2 K4 Eu1 35.58(9) 1_655 1_655 ?
O1 K4 Eu1 81.77(10) 2_655 1_655 ?
O1 K4 Eu1 35.38(9) 3_655 1_655 ?
O2 K4 Eu1 90.00(9) 3_655 1_655 ?
O2 K4 Eu1 157.28(10) 2_655 1_655 ?
Si1 K4 Eu1 91.30(3) 3_655 1_655 ?
Si1 K4 Eu1 145.21(8) 2_655 1_655 ?
Eu1 K4 Eu1 67.83(4) 4_665 1_655 ?
F1 K4 Si4 117.90(10) 3_655 2_655 ?
O2 K4 Si4 81.22(10) 4_665 2_655 ?
O2 K4 Si4 130.59(12) 1_655 2_655 ?
O1 K4 Si4 21.92(9) 2_655 2_655 ?
O1 K4 Si4 84.18(11) 3_655 2_655 ?
O2 K4 Si4 129.43(11) 3_655 2_655 ?
O2 K4 Si4 60.08(9) 2_655 2_655 ?
Si1 K4 Si4 106.22(7) 3_655 2_655 ?
Si1 K4 Si4 45.39(4) 2_655 2_655 ?
Eu1 K4 Si4 54.81(3) 4_665 2_655 ?
Eu1 K4 Si4 100.90(6) 1_655 2_655 ?

_diffrn_measured_fraction_theta_max 0.995
_diffrn_reflns_theta_full        25.14
_diffrn_measured_fraction_theta_full 0.995
_refine_diff_density_max         0.980
_refine_diff_density_min         -0.938
_refine_diff_density_rms         0.174
_database_code_depnum_ccdc_archive 'CCDC 1007246'
